Device application of low-temperature-grown Al(0.3)Ga(0.7)As: GaAs microwave power field effect transistorкод для вставкиСкачать
INFORMATION TO USERS This manuscript has been reproduced from the microfilm master. UMI films the text directly from the original or copy submitted. Thus, some thesis and dissertation copies are in typewriter face, while others may be from any type of computer printer. H ie quality of this reproduction Is dependent upon the quality of the copy submitted. Broken or indistinct print, colored or poor quality illustrations and photographs, print bleedthrough, substandard margin^ and improper alignment can adversely afreet reproduction. In the unlikely event that the author did not send UMI a complete manuscript and there are missing pages, these will be noted. Also, if unauthorized copyright material had to be removed, a note win indicate the deletion. Oversize materials (e.g., maps, drawings, charts) are reproduced by sectioning the original, beginning at the upper left-hand comer and continuing from left to right in equal sections with small overlaps. Each original is also photographed in one exposure and is included in reduced form at the back of the book. Photographs included in the original manuscript have been reproduced xerographically in this copy. Higher quality 6” x 9" black and white photographic prints are available for any photographs or illustrations appearing in this copy for an additional charge. Contact UMI directly to order. UMI A Bell & Howell Information Company 300 North Z eeb Road. Ann Arbor. Ml 48106-1346 USA 313/761-4700 800/521-0600 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. UNIVERSITY OF CALIFORNIA Santa Barbara Device Application o f Low-Temperature-Grown Alo.3Gao.7As: GaAs M icrowave Power Field Effect Transistor A Dissertation submitted in partial satisfaction o f the requirements of the degree of Doctor of Philosophy in Electrical and Computer Engineering by Nguyen Xuan Nguyen Committee in charge: Professor Umesh K. Mishra, Chairperson Professor Arthur C. Gossard Professor Evelyn L. Hu Professor Herbert Kroemer June 1997 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. UMI N u m b e r: 9 8 0 0 4 7 9 UMI Microform 9800479 Copyright 1997, by UMI Company. All rights reserved. This microform edition is protected against unauthorized copying under Title 17, United States Code. UMI 300 North Zeeb Road Ann Arbor, MI 48103 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. The Dissertation o f Nguyen Xuan Nguyen is approved: Professor Arthur C. Gossard Professor Evelyn L. Hu Professor Herbert Kroemer Professor Umesh K. Mishra - Chairperson March 1997 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. Copyright by Nguyen Xuan Nguyen 1997 iii Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. ACKNOWLEDGEMENTS I would like to sincerely thank many people who have made my years of graduate study at UCSB memorable ones. The friendly and cooperative atmosphere fostered by the faculty in the ECE department has been very conducive to research and learning. The excellent facilities and supports provided by the staff made my research possible. In particular, I would like to express my sincerest gratitude to Professor Mishra for his guidance and support. I am grateful to the members of my committee, Professors Hu, Gossard, and Kroemer for their suggestions and interest in this project. Many thanks are due to Jack Whaley, Brian Carrelejo and Tom Reynolds for the maintenance o f the equipment and for providing the quick fixes to the clean-room problems. I would like to thank Lie-Wei Yin for introducing me to GaAs MESFET processing. Thanks are due to James P. Ibbetson, Wei-Nan Jiang, and Prashant Chavarkar for the many discussions on MBE growth and materials, moreover for providing me all the epitaxial samples critical in my research. I am also indebted to the Kellers, Bemd and Stacia, for their expertises in MOCVD selective regrowth of GaAs. Special thanks are due to the former and current occupants of the microwave/millimeter wave lab: Gil Chinn for the white noises, Jon Lynch for the caffeine kicks, Jeff Yen for the voice simulations and jokes, Angelos Alexanian for the chocolate covered prunes! Kursad Kiziloglu for the use of his mini-library, Robert Underwood for the exchanges and tips on computers; Jeff Shealy, Primit Parikh, Yifeng Wu, Amit Nagra for the discussions on processing and device measurements. Last but not least, I would like to thank Chanh Nguyen, Ginger Yu and David Holcombe for their constant friendship over the years. iv Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. Dedicated to my parents Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. VITA September 5th, 1968 - Bom in Saigon, Vietnam 1990 - B. S. E. E., University o f California, Santa Barbara 1992 - M. S. E. E., University o f California, Santa Barbara PUBLICATIONS 1. N. X. Nguyen, K. Kiziloglu, J. P. Ibbetson, L.-W. Yin, M. M. Hashemi, and U.K. Mishra, "The Output Conductance in GaAs Air-Gap MESFETs", Technical Digest, 50th Annual Device Research Conference, Cambridge, MA, USA, 22-24, June 1992 IEEE Trans, on Electron Devices, E D -39,2649 (1992) 2. L.-W. Yin, N. X. Nguyen, Y. Hwang, J.P. Ibbetson, R. M. Kolbas, A. C. Gossard. and U. K. Mishra, "Temperature Investigation o f the Gate-Drain Diode of Power GaAs MESFET with Low-Temperature-Grown (Al)GaAs Passivation", Journal of Electronic Materials,V22, No. 12, 1503 (1993) 3. J. P. Ibbetson, J. S. Speck, N. X. Nguyen, A. C. Gossard, and U. K. Mishra "The Role o f Microstructure in the Electrical Properties o f GaAs Grown at Low Temperature", Journal of Electronic Materials, V22, No. 12 , 1421(1993) 4. L.-W. Yin, N. X. Nguyen, K. Kiziloglu, J. P. Ibbetson, A. C. Gossard, and U. K. Mishra, "Device Performance of Submicrometre MESFETs with LTG Passivation", Electronics Letters, V29, No. 17, 1550 (1993) 5. N. X. Nguyen, J. P. Ibbetson, J. C. Yen, M. M. Hashemi, and U. K. Mishra "Encapsulated GaAs Power MESFET", Proceedings IEEE/Cornell Conference on Advanced Concepts in High Speed Semiconductor Devices and Circuits, Cat. No. 93CH32359, Aug. 2-4, 1993 vi Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. 6. W.-N. Jiang, N. X. Nguyen, R, D. Underwood, and U. K. Mishra, "Telluriumdoped Al0 .4 3 Ga0 .5 7 As/(In 0 .2 )GaAs Modulation Doped Heterostructures by Molecular -Beam-Epitaxy", Applied Physics Letters, V 6 6 , No. 7, 845(1995) 7. N. X. Nguyen, W.-N. Jiang, K. A. Baumann and U. K. Mishra, "High Breakdown AlGaAs/InGaAs/GaAs PHEMT with Tellurium doping", Electronics Letters, V31, No. 7, 586(1995) 8. N. X. Nguyen, J. P. Ibbetson, W.-N. Jiang, and U. K. Mishra "Low Temperature Grown AlGaAs Passivation in GaAs Power MESFETs", Proceedings IEEE/Comeli Conference on Advanced Concepts in High Speed Semiconductor Devices and Circuits, Cat. No. 95CH35735, Aug. 7-9, 1995 9. C. Nguyen, T. Liu, H.-C. Sun, M. Chen, D. Rensch, N. X. Nguyen, and U. K. Mishra "Current Transport in Band-Gap Engineered AlInAs/GalnAs/InP Double Heterojunction Bipolar Transistor Using Chirped Superlattice", Proceedings IEEE/Cornell Conference on Advanced Concepts in High Speed Semiconductor Devices and Circuits, Cat. No. 95CH35735, Aug. 7-9, 1995 10. N. X. Nguyen, J.P. Ibbetson, and U. K. Mishra "Interfacial Barrier of LTGAlo. 3 Gao.7 As Epitaxial Passivation in GaAs FETs", presented at the 1996 Electronic Material Conference, Santa Barbara, CA, June 26-28. 11. N. X. Nguyen, J. P. Ibbetson, and U. K. Mishra "GaAs Power FET with LowTemperature-Grown Alo.3 Gao.7 As Passivation" submitted for publication in Electronics Letters 1997 12. N. X. Nguyen and U. K. Mishra "Uses of Low Temperature Grown Materials in MESFETs", DataReviews INSPEC, March 1996 vii Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. ABSTRACT Device Application o f Low-Temperature-Grown Alo.3Gao.7As: GaAs Microwave Power Field Effect Transistor by Nguyen Xuan Nguyen The performance, uniformity and therefore the cost of reliable GaAs power FETs have been limited by the non-reproducibility of the gate diode characteristics. The main reason for this is the lack o f an effective electrical passivation o f the GaAs surface adjacent to the gate. In this research project, we have investigated the application o f low-temperature-grown (LTG) Alo.3Gao.7As as an electrical passivation layer for GaAs FETs. In particular, the surface layer engineering to improve breakdown voltage o f GaAs FETs with LTG- Alo.3Gao.7As is systematically studied. Drawing from the established material properties of LTG-GaAs, a simple model is proposed to explain the physical mechanism through which the LTG materials passivation alleviate peak field in a MESFET structure. The unique existence o f the natural compensated deep donors in LTG materials is believed to be responsible for the improved breakdown voltage of LTG passivated devices. Two dimensional device simulation to confirm this model has been performed. A systematic study of the effect of growth and annealing temperatures on LTG-Alo.3 Gao.7As passivated M E S F E T s has been performed. Breakdown voltage and low frequency noise characteristics o f the devices are foound to be critically dpended on both the growth and annealing temperatures. A high performance GaAs-based power MESFET which incorporates an L T G -A lo jG a 0 7As passivation is demonstrated. Record power performance of 1.0 W/mm at 30% power-added-efficiency (PAE), and 0.5 W/mm at 46% PAE has been achieved. These results provide clear testimony for the potential o f the L T G -A I0 3Ga . AS 0 7 passivation technology for microwave power FETs. viii Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. Table of Contents 1. Introduction 1.1 Overview....................................................................................................... 1 1.2 High Power GaAs FET.............................................................................. 4 1.3 Effect o f Surface Condition on Breakdown Voltage................................ 6 1.4 Scope o f Dissertation..................................................................................9 1.5 References....................................................................................................11 2. Electrical Properties o f Low Temperature Grown Material 2.1 Introduction................................................................................................. 13 2.2 LTG-GaAs Material Properties................................................................ 14 2.3 LTG-Alo.3Gao.7As Material Properties.....................................................18 2.4 Interfacial Property o f LTG-Alo.3 Gao.7As Passivation.......................... 20 2.4.1 Basic Concept o f Experiment......................................................22 2.4.2 Effect o f Growth and Annealing Temperatures....................... 24 2.5 Summary..................................................................................................... 29 2.6 References................................................................................................... 31 3. Surface Layer Engineering to Improve Breakdown Voltage 3.1 Introduction................................................................................................. 34 3.2 Breakdown Voltage in GaAs Power M ESFET....................................... 35 3.3 Breakdown Voltage Improvement by LTG Materials Passivation 38 3.4 Two Dimensional Electrostatic Simulation o f LTG-GaAs Passivation 3.4.1 Basic Semiconductor Equations................................................ 42 3.4.2 Simulation Results and Analysis.................................................43 3.5 Summary......................................................................................................49 3.6 References....................................................................................................51 ix Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. 4. Experimental Implementation of LTG-GaAs Passivation 4.1 Introduction................................................................................................. 53 4.2 Device Design and Fabrication.................................................................. 54 4.3 Device Results and Analysis 4.3.1 Characteristics o f Devices with Unanealed LTG- Al03Ga07As Passivation............................................................................................ 58 4.3.2 Effect o f Annealing on Gate-Drain Breakdown Voltage..........59 4.3.3 Effect o f Annealing on Low-Frequency Noise........................... 62 4.4 Summary......................................................................................................67 4.5 References.................................................................................................... 6 8 5. High Performance GaAs Microwave Power FET 5.1 Introduction..................................................................................................70 5.2 Device Design and Fabrication................................................................... 70 5.3 Device Result and Analysis 5.3.1 DC Characteristics...................................................................... 73 5.3.2 RF Characteristics....................................................................... 76 5.3.3 Microwave Power Performance................................................. 77 5.4 Summary...................................................................................................... 80 5.5 References.................................................................................................... 81 6. Summary and Future Work Summary............................................................................................................ 83 Suggestion for Future W ork............................................................................. 85 References..........................................................................................................87 x Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. CHAPTER 1 Introduction 1.1 O verview : The advent of the commercial wireless communication market has brought forth new demands for compact, low cost, and high performance microwave components and systems. This in turn leads to a demand for low cost and high performance microwave semiconductor circuits and devices. In particular, there are pressing needs for semiconductor devices that have high raw microwave power, high linearity, and high efficiency. Recent developments in compound semiconductor materials and technology have led to the popular belief that compound semiconductor devices would provide the answers to these stringent demands of the industry. In particular, Gallium Arsenide MEtal Semiconductor Field Effect Transistor (GaAs MESFET) has been demonstrated to have the potentials of meeting the demand of both low cost and high performance [1-3]. The maturity and simplicity of the GaAs MESFET fabrication technology have led to the establishment of this device and its variation as the work horse of the compound semiconductor industry . However, as of present, GaAs MESFET has been plaqued by a simple, yet detrimental problem that has inhibited its widespread usages - low yield . Over the years, studies have led to the conclusion that the main culprit of the low yield problem in GaAs devices is the non-uniform native oxide formed on top of the GaAs surface when it is expose to atmospheric ambient [5-7]. This native oxide depended sensitively on the processing treatments that the samples underwent in the device fabrication procedure, which led to the high device-to-device 1 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. non-uniformity and low run-to-run reproducibility. This problem has been continually studied and addressed by material scientists and device engineers through various approaches. To date, the most promising solutions have came from chemical treatments o f the GaAs surface. Photochemical oxidation and sulfide chemical passivation such as Na,S and (NH4)2S [8 , 9] have demonstrated to be the most promising solutions. However, the drawback o f these chemical treatments technology is that they leave the GaAs surface susceptible to thermal and environmental instabilities; therefore device reliability remained an issue. From a device engineeriing point of view, the problem of low yield in GaAs devices could alternatively be addressed through the development of a stable and effective electrical passivation technology for GaAs materials and devices. As shown in Figure la and lb, an ideal electrical passivant layer should have the following properties: (i) It should maintain (or increase) the breakdown voltage of the FET. (ii) It should effectively screen the channel from the surface of the device to lower 1/f noise, critical in linear communication systems. (iii) It should not deplete the underlying channel thereby increasing channel resistance and losses (decreasing efficiency). This property can be alternatively stated as ‘the interface potential difference between the passivant and the channel should be low.’ (iv) It should not increase the gate leakage. Recent advances in a new kind of molecular beam epitaxial (MBE) materials, known as Low-Temperature-Grown (LTG) GaAs and related materials, have been shown to have the potentials of satisfying all of the stated above properties of an ideal passivation layer. The goal of the present research project is to gain definitive 2 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. understandings into the device application of LTG materials as an electrical passivation technology; and to further the use of LTG materials as a tool for device engineering to improve breakdown voltage and power performance. decoupling of the channel and the surface SO U RCE DRAIN GATE Epitaxial Passivation Low <P (interfacial potential): low parasitic resistance alleviation of peak gate Geld n-GaAs channel (a) deep d o n o r: low free electron concentration LTG Passivation n-GaAs channel depletion region (o r screening depth) (b) Figure 1.1: (a) Schematic FET showing important parameters to consider when choosing a surface passivant. (b) Schematic band diagram through gate, passivant and channel of device. Chapter I sets the tone and provides the general background for the remainder of the dissertation. In the next two sections of this chapter, issues and problems in GaAs power MESFET are reviewed; in particular, the important relationship between 3 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. surface conditions and breakdown in field effect transistors will be discussed. The chapter then concluded with the last section summarizing the scope of the present dissertation. 1.2 High Power GaAs FET : Maximum output power in microwave device shares a similar motive as speed in digital integrated circuits - the more, the better. As such, it is highly desirable to maximize the power performance of microwave device in general, and of GaAs FET in particular. The first realization of high power GaAs FET were reported simultaneously by Fukuta et al  and Napoli eta l  in 1973. Since then, intense efforts had been devoted into maximizing the output power obtainable from GaAs field effect transistors. Figure 1.2 summarized some of the annual progress in the output power of GaAs FET reported. For high power application, a device must be able to sustain both high voltage and current in order to convert the DC power into microwave or millimeter-wave power. Proper device design of a high power GaAs MESFET required close attentions to various cross-linked design parameters such as doping density profile, channel thickness, and geometric layout, etc. The correlations between these design considerations and the related performance indicators are briefly summarized in Table 1.1. 4 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. 1978 1988 1987 1976 3 O CL i □L 3 a3 o 1983 0.1 1 2 3 5 10 20 50 100 Frequency f (GHz) F ig u re 1.2: Progress in microwave power performance of GaAs FETs - the First practical GaAs power FET was reported in 1973 . Table 1.1: Microwave power FETs design parameters and figures-of-merit. Design P aram eter C haracteristics Pow er Performance Doping Density Drain Current Output Power Epitaxial Thickness Transconductance Gain Geometric Spacings Gate Breakdown Efficiency Gate Length Parasitic Resistances Distortion Ohmic Contacts Knee Voltage Cutoff Frequency Surface Passivation Reliability Metallization A nominal class-A bias configuration of a FET for power application is shown in Figure 1.3. As indicated in the figure, the maximum output power of a device is 5 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. directly proportional to both the maximum drain current and the breakdown voltage. Although, at a first glance, the drain current of the device is a function of just the channel doping and thickness; however, on closer examination of the limitation of its maximum drain current, we immediately see that the maximum drain current is dictated by the criteria that it could be completely pinch-off, prior to breakdown. Therefore, the maximum drain current is also indirecdy governed by the breakdown of the device. In short, the breakdown voltage is of paramount importance in the power performance of a FET. For GaAs MESFET, work over the years have clearly demonstrated that its breakdown voltage critically depended on the surface condition [6 , 1 1 , 1 2 ], and in particular the surface condition in the vicinity of the gate. Class A bias loaddine BV Figure 1.3: Nominal class-A bias configuration of a GaAs power field-effect transistor. The load-line is shown for maximum output power condition, which is directly proportional to the maximum drain current and the breakdown voltage. 1.3 Effect o f Surface Condition on Breakdown Voltage: Under nominal bias for microwave power application, the gate-drain region of a MESFET structure sustained the highest potential difference. This potential difference resulted in a local high field region; which in turn led to the eventual breakdown of the device. Direct experimental observations of light emissions from 6 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. this high field region have pinpointed its locale at the drain edge of the gate [13, 14]. Therefore, the breakdown voltage of a FET could be increased by one of two means, either by reducing the peak electric field at the gate and/or reducing the injected electron density (gate leakage) which reduces multiplication in the channel. The latter can be achieved independently of the former by inserting a wide band gap material under the gate metal (ie, a Metal Insulator Semiconductor FET, MISFET, structure). The former is the focus of the present research. Any advances made with this approach can also be applied to MISFETs structure for added benefit. Reducing the electric field at the gate can also be achieved in two ways, schematically shown in figures 1.4a and 1.4b. The first is by distributing the potential between the gate and the drain by adding a shunt resistive path to the channel. Here, in the simplest case, the linear increase in voltage along the resistor is reflected in the channel through the barrier height of the resistor on the semiconductor. The disadvantage of this technique is that the ladder network is a low pass filter. Beyond the cut-off frequency, the effectiveness of the network in redistributing the surface potential rolls off and hence the breakdown voltage of the device decreases with frequency, beyond the pole of the network. The second means of alleviating the peak electric field, illustrated in figure 1.4b, is by allowing tunnel injection of charge from the drain edge of the gate into states in the passivant close to the gate. Again, this approach may have some frequency dependence related to the capture and emission times from the traps. LTG materials passivation, in particular LTG-GaAs and LTG-AlGaAs, with the appropriate growth and annealing conditions, are capable of providing electrical characteristics that resulted in either of the two field alleviation mechanisms stated. Therefore, the 7 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. engineering o f this materials to tailored their parameters to obtain the desire electrial passivation properties is of great practical interests. DRAIN GATE AAAt t VW V n-GaAs channel (a) SOURCE DRAIN GATE Q-CUB TG;(Al)GaAs n-GaAs channel Buffer-GaAs (b) Figure 1.4: Field alleviation by a) voltage redistribution through an RC ladder network and b) by charge injection into the LTG material in the vicinity of the gate. 8 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. 1.4 Scope o f D issertation: As common in the early stage of the research and development for most new materials, there usually existed a vast body of empirical data and reports on the material properties and also different models to explain these properties, some are even in contradiction with others; LTG materials and its applications are no exception to this rule. While this pose no serious problem in the research of the material science of LTG materials, it brought about many unresolved issues and potential contradictions in the paralleled device research based on the new material. Questions such as “What are the relevant material properties to device applications?” required constant attentions. The main focus of Chapter 2 is the established material properties of LTG materials that directly related to electronic devices. Other issues, such as the temperature dependence passivation properties of LTG materials such as channel band bending are also investigated and discussed. Chapter 3 draws on the LTG material properties to explain the effect that LTG passivation has on the breakdown voltage of GaAs FET. In particular, a physical model of the field alleviation by LTG materials passivation, through the compensated deep donors, is proposed. Two dimensional electrostatic simulations of the device are performed to verify the model. Chapter 4 focuses on the experimental implementation of LTG-Al03 Ga07As passivation in actual devices. The effects of growth temperatures and subsequent annealing treatment o f LTG-AI0 3Gao 7As on the breakdown voltage and other device characteristics are studied. Chapter 5 presents the characteristics and performance of a high-power GaAs heterostructure field effect transistor that has incorporated an LTG-AI^Ga^As 9 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. electrical passivation layer. Record power performance at C-band are presented and discussed. Chapter 6 concludes the present dissertation with a summary of research conclusions and recommendation for some possible revenues of future research. 10 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. 1.5 R eferences:  M. Fukuta, T. Mimura, I. Tsujimura, and A. Furumoto, “Mesh source type microwave power FET,” IEEE International Solid State Circuit Conference Technical Digest, pp. 84-85, 1973.  A. Higashisaka, Y. Takayama, and F. Hasegawa, “A high-power GaAs MESFET with an experimentally optimized pattern,” IEEE Transactions on Electron Devices, Vol. 27, pp. 1025-1029, 1980.  Y. Aokie and Y. Hirano, High-power GaAs FETs. Boston London: Artech House Inc., 1993.  H. Fukui, S. H. Wemple, J. C. Irvin, W. C. Nehaus, J. C. M. Hwang, H. M. Cox, W. O. Schlosser, and J. V. DiLorenzo, “Reliability of power GaAs field-effect transistors,” IEEE Transactions on Electron Devices, Vol. 29, pp. 395-401, 1982.  W. R. Frensley, “Power-limiting breakdown effects in GaAs MESFETs,” IEEE Transactions on Electron Devices, Vol. 28, pp. 962-970, 1981. [6 ] H. Mizuta, K. Yamaguchi, and S. Takahashi, “Surface potential effect on gate-drain avalanche breakdown in GaAs MESFETs,” IEEE Transactions on Electron Devices, Vol. 34, pp. 2027-2033, 1987.  T. M. Barton, “Simulation of surface state dynamics on GaAs MESFETs,” European Transactions on Telecommunications and Related Technologies. Vol. 1, pp. 393-400, 1990. Reproduced with permission of the copyright owner. Further reproduction prohibited without permission.  R. S. Besser and C. R. Helms, “Comparison of surface properties of sodium sulfide and ammonium sulfide passivation of GaAs,” Journal o f Applied Physics, Vol. 65, pp. 4306-4310, 1989.  E. Yablonovitch, B. J. Skromme, R. Bhat, J. P. Harbison, and T. J. Gmitter, “Band bending, Fermi level pinning, and surface fixed charge on chemically prepared GaAs surfaces,” Applied Physics Letters, Vol. 54, pp. 555-557. 1989.  L. S. Napoli, R. E. DeBrecht, J. J. Hughes, A. Dreeben, and A. Triano, “High power GaAs FET amplifier - a multigate structure,” IEEE International Solid-State Circuti Conference Technical Digest, pp. 82-83, 1973.  T. M. Barton and P. H. Ladbrooke, “Dependence of maximum gate-drain potential in GaAs MESFET’s upon localized surface charge,” IEEE Electron Device Letters, Vol. 6, pp. 117-119, 1985.  T. M. Barton and P. H. Ladbrooke, “The role of the device surface in the high voltage behaviour of the GaAs MESFET,” Solid-State Electronics, Vol. 29, pp. 807-813, 1986.  T. Mimura, H. Suzuki, and M. Fukuta, “Visible light emission from GaAs field-effect transistor,” Proceedings o f the IEEE, Vol. 65, pp. 1407-1408, 1977.  H. Q. Tsemg, W. R. Frensley, and P. Saunier, “Light emission of GaAs power MESFETs under rf drive,” IEEE Electron Device Letters, Vol. 1, pp. 20-21, 1980. Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. CHAPTER 2 Electrical Properties o f Low Temperature Grown Materials 2.1 Introduction: Device application was the initial driving force in the research and development o f low-temperature-grown (LTG) GaAs; and ever since, it has paralleled and complemented the material research of LTG-GaAs and related compounds. The first interest in the device application of LTG material dated back to February 1988 in a paper published by Smith et al , where LTG-GaAs was first demonstrated to be an effective buffer for the reduction o f backgating in GaAs IC. This first demonstration o f the beneficial effect of LTG-GaAs has since generated a flurry of activity in the quest for more understandings of the material properties and other potential device applications of LTG materials. Soon afterward, another device application o f LTG-GaAs was reported. The utilization o f annealed LTG-GaAs as a surface insulator in a MISFET structure to improve the gate-drain breakdown voltage was demonstrated by Yin et al  in 1990. This new technology, LTG materials passivation, caught the interests of device engineers because it provides a new tool in dealing with a long standing problem of surface passivation in GaAs devices. The strong dependency o f the LTG material properties on its synthesis condition allowed them to be readily engineered to yield desired device characteristics. These preliminary device results demonstrated the potential of this new LTGGaAs passivation technology in GaAs FET. However, as with any new technology, new questions arose, and satisfactory answers to them required further investigations and understanding. Questions such as, “What are the unique properties of the LTG materials? How does LTG passivation effect other device characteristics? And what 13 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. parameters can we engineer to optimize the device performance?” points to a need for better understanding o f the material properties and their correlations to the synthesis process involved. To date, over two hundred papers have been published on the various properties and models o f LTG-GaAs and related materials; some even with conflicting reports, on the properties o f LTG materials. As such, it would be beyond the scope of a single chapter in a thesis to provide a comprehensive review of the various reported properties o f LTG materials in literature. The objective of the present chapter is to provide a focused summary and review o f the LTG material properties that are pertinent to electronic devices,; and also to present some experimental data that had been obtained recently on the interfacial properties o f the LTG-Alo.3 Gao.7 As passivation layer to the underlying normal materials. The next section focuses on the current established material properties and understanding o f LTG-GaAs. This is followed by a section on the reported properties of LTG-Alo.3 Gao.7 As. The last section of the chapter presents the results of our recent experimental study on the interfacial property o f the LTG-Alo.3 Gao.7 As passivation layer and the GaAs channel. In particular, the parameter space of the channel band-bending as a function of growth and annealing temperatures of the LTGAlo.3 Gao.7 As layer have been systematically investigated. This parameter is o f great interest in the design o f devices with LTG-Alo.3 Gao.7 As passivation. 2.2 LTG-GaAs Material Properties: The unique synthesis characteristics o f LTG-GaAs is explicitly stated in its acronym, low temperature grown. Unlike conventional molecular beam epitaxy of GaAs, which is nominally grown at substrate temperatures o f 580-600°C, LTG-GaAs is grown at a substrate temperature of ~200°C. With all other growth parameters 14 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. (beam equivalent pressure and growth rate) similar to that o f normal GaAs, this difference in growth temperature alone has resulted in spectacularly different electrical and optical properties o f the materials. The exact growth temperature (in the 200°C range) has been observed to intimately influence both structural and electrical properties o f the LTG-GaAs film. Analysis o f as-grown LTG-GaAs has revealed that the material contains a large concentration o f excess As, between 1-2% (10 2 °-10 21 excess As atoms per cm3), which renders the material non-stoichiometric. The amount of excess As depends strongly on the growth temperatures of the GaAs film . Initially, this excess As is incorporated into the GaAs lattice primarily as point defects such as As antisites (AsQa)  and possibly As interstitials (Asi) . These defects are believed to be responsible for the observed expansion of the GaAs lattice. Electron paramagnetic resonance (EPR) [6 ], near infrared absorption (NIRA) , and magnetic circular dichroism absorption (MCDA)  experiments have positively identified that AsGa is the main contributor to the observed donor-like point defects in LTG-GaAs. The average concentration of this donor-like defect is about 102 0 cm*3 for samples grown at ~200°C and decreases monotonically to about 1018 cm*3 for those grown at higher temperatures (>300°C). Extraction of the activation energy o f this AsGa_related donor from an Arrhenius plot yields an energy of 0.65 ± 0.01 eV [8 ]. In addition to the As antisite defect, there is also evidence of another donor-like defect, the As interstitial defect; however this defect is believed to be electrically inactive [8 ], thus it has not received much attention. In addition to these two donor-like defects, from stoichiometry consideration, another defect is assumed to exist in large quantity in LTG-GaAs, the gallium vacancy defect (VQa)- Unlike the first two defects, the VQa defect is acceptor-like. It is 15 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. believed to be the source o f the large concentration o f acceptors observed in the material. Preliminary data from absorption studies and thermally stimulated current experiments have yielded a concentration o f1 0 19 cm-3, with an energy level of 0.27 ± 0.3 eV above the valence band for the VGa point defect . The high concentration o f both deep donors and deep acceptors in the asgrown LTG-GaAs results in a compensated deep donor level in the material. Electrically, this compensated deep donor provided a path for hopping conduction of carriers under applied bias. Therefore, as-grown, LTG-GaAs is generally conductive, with resistivity o f the order of 10 Q-cm [ 1 0 ]. Upon annealing at high temperature (>400°C), a dramatic change in the material properties o f the LTG-GaAs is observed. The film usually relaxes and the lattice constant returns to that found in normal GaAs. The initial excess arsenic in the film (Asi and AsQa) diffuses and clusters together to form As precipitates. Scanning tunneling microscopy (STM) studies of these precipitates have revealed several structures, from an amorphous structure for smaller size (diameter of 20-30A) to hexagonal for larger size ( >40A) . Annealing at higher temperatures results in larger precipitates but lowers total precipitate density in the material. In addition, annealing also has dramatically reduced the concentration o f both AsGa and VGa point defects in the LTG-GaAs layer. A recent systematic measurement of these defects as a function of growth and annealing temperatures is shown in figures 2 .1 16 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. Growth T (°C) 280 260 240 220 200 1.0 o o 1 0.1 I 1.9 1.8 ?• So *3 • from MCOA ° from NIRA , 1 2 2.1 1000/r (1/K) (a) Annealing T (.°C) 800 600 / LT GaAs c o <3 ^ 1.0 §O E O r Ea-1.3eV./ / So c o ------A t- u grown; Y 1 .•o ' |2 J 'Ea»1.4eV • from UCDA. o from NIRA 0.1 Sfp ©E y cs oC3OC < 200 400. J 0.8 1.0 1.2 1.4 1.6 1.8 2.0 2.2 1600rr (1/K) (b) Figure 2.1: Defects concentrations in LTG-GaAs as a function o f (a) growth and (b) annealing termperatures. The charged AsGa were measured by MCDA and the neutral AsGa by NIRA. The charged AsGa concentration can be view as an indirect measurement of the deep acceptors concentration in the materials, while the sum of both charged and neutral AsGa is equivalent to the total deep donors concentration Electrically, annealing at high temperatures drastically changes the resistivity of the LTG-GaAs layer. The resistivity increased from 10 Q-cm in the as-grown LTG-GaAs to 106 Q-cm in the LTG-GaAs annealed at 600°C for 10 minutes. This strong dependence of resistivity on the annealing temperatures o f LTG-GaAs and the mechanisms responsible for it have attracted a lot of attentions from material 17 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. scientists and engineers in recent years. A summary of the dependence o f resistivity o f LTG-GaAs on the growth and annealing temperatures is shown in figure 2.2 . o 107 o e 106 s CL 104 103 • o 102 10’ - i — i 200 300 - - • as-grown O annealed (590 *C. 10 min) - i — - * 400 t 500 600 Tg CC) Figure 2.2: Room temperature resistivities as a function of growth temperatures for as-grown and annealed GaAs MBE layers [From  ]. The microscopic picture of the origin of this unique LTG materials characteristics has been and still is a lively topic o f debate among workers in the field. As o f present, the two contending models for this unique property of LTG-GaAs are: the As precipitate dominated model and the point defects dominated model. To date, there is insufficient evidence to assert the correctness of one model over the other, and it is generally agreed that further investigations are needed before definitive conclusions could be drawn. 2.3 LTG-Alo.3 Gao.7 As M aterial Properties: With LTG-GaAs demonstrating many unique and interesting material properties, especially the high resistivity and high breakdown field strength of annealed LTG-GaAs, it was natural for researchers to investigate other low 18 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. temperature grown III-V compounds and their potentials. Low temperature grown materials such as InxGai-xAs [13, 14], InP [15, 16], AlxGai.xAs , and InGaP  have been studied and reported. In particular, LTG-Alo.3 Gao.7 As has attracted much attention from device engineers because o f its close resemblance to LTG-GaAs, but with an added advantage o f a larger bandgap. This mean that LTG-Alo.3 Gao.7 As can also be engineered to be utilized in applications similar to LTG-GaAs, but with additional benefits. The larger bandgap o f the Alo.3 Gao.7 As material should further improve the material breakdown field strength and also yield higher resistivity. Preliminary reports o f the properties o f LTG-Alo.3 Gao.7 As show that this is indeed the case. LTG-Alo.3 Gao.7 As is grown at a substrate temperature of about 250°C, about 50°C higher than LTG-GaAs. The slightly higher substrate temperature is required to retain good crystallinity o f the Aluminum containing compound. Structurally, LTGAlo.3 Gao.7 As is reported to be similar to LTG-GaAs: the as-grown samples contain an excess concentration o f As, and upon annealing at high temperatures, As precipitate formation is observed. However, for the same annealing temperature, the precipitate size and density are lower for LTG-Alo.3 Gao.7 As than that found in LTGGaAs. Electrical characterization o f LTG-Alo.3 Gao.7 As film utilizing a metalinsulator-semiconductor (MIS) structure yielded a resistivity of 1.8X104 Q-cm and 6x10’ 1 Q-cm for unannealed and 600°C annealed films, respectively. This resistivity is about three orders o f magnitude higher than that found in LTG-GaAs. A study of the transport through annealed LTG-Alo.3 Gao.7 As film, using an n-LTG-n structure, revealed that similar to LTG-GaAs, low fields the conduction is dominated by hopping conduction through a defect band; and at high field, is space charge limited. 19 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. Temperature-dependent conductivity measurements have identified a donor-like defect with an activation energy of 0.96 ± 0.03 eV . Drawing from the similarity between the structural and transport property o f LTG-Alo.3 Gao.7 As to that o f LTGGaAs, it is expected that point defects, such as AsQa, Asi and VQa exist in LTGAlo.3 Gao.7 As with comparable quantity. However, systematic measurements of exact concentrations and associated energy levels o f these defects still await further studies. In the next section o f the chapter, a material property that has direct bearings on the application o f the material to devices, its interfacial property, has been investigated. The dependence o f the interfacial property, such as the band-bending, as a function o f growth and annealing temperature is reported. Drawing from the reported bulk material properties of the previous two section, a simple hypothesis for the behavior o f the band-bending is proposed. The work in this next section was undertaken at UCSB by the author, with the assistance of James Ibbetson in the sample growth and transmission electron microscopic work. 2.4 Interfacial Property of LTG-AIo.3 Gao.7 As Passivation: The strong dependence o f material properties on the processing parameters, growth and annealing temperatures, of LTG materials lends itself naturally to the engineering o f the materials in device application. In particular, the high resistivity and high breakdown field strength of LTG-Alo.3 Gao.7 As make it a potential ideal electrical passivation layer for GaAs device and materials. However, initial efforts to incorporate such passivation layer into a field effect transistor device structure were hampered by a detrimental diffusion of defects and precipitates into the channel during the annealing process of the LTG layers. This diffusion, in turn led to a strong depletion o f the carriers in the channel and rendered the channel useless. However, a solution to this problem was soon found - an insertion of a thin undoped AlAs layer 20 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. between the LTG passivation layer and the active channel o f the device would protect the active channel effectively . The AlAs diffusion barrier, o f thickness between 100A to 200A, has shown to be effective up to annealing temperature o f ~650°C. Recently, other effective diffusion barriers of different materials such as InGaP and AlGaAs/GaAs superlattices have also been reported [2 1 ]. While the diffusion barrier has been sufficient in preserving the integrity of the active layer in a device, and therefore allowing the successful incorporation of LTG materials into device structures, it has also brought about other technological issues that raised other concerns. In particular, for LTG-Alo.3 Gao.7 As, the thin AlAs diffusion barrier layer had led to an intriguing observation at the interface o f the LTGAlo.3 Gao.7 As and itself. This phenomenon is best illustrated in a cross-sectional transmission electron micrograph of a nominal device structure, as shown in figure 2.3. Clearly observable in the figure, the interface o f LTG-Alo.3 Gao.7 As and AlAs is decorated with a much higher concentration of As precipitates in comparison to that found in the bulk o f the LTG-Alo.3 Gao.7 As layer on top, and the underlying active channel is precipitate free. From a device standpoint, the observed accumulation of excess As precipitates at the interface raises question about its effect on the device characteristics and performance. In addition, since the properties o f LTG-Alo.3 Gao.7 As are strongly dependent on the growth and annealing temperatures; the effect of these process parameters on the interface, and in turn on device characteristics, is o f great importance. A clear understanding and handle on these effects would yield valuable insights into the suitability o f LTG-Alo.3 Gao.7 As as a passivation layer for GaAs field effect transistors. In this work, a focused empirical study o f the interfacial 21 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. barrier, or more accurately the channel band-bending, as a function of the growth and annealing temperature space has been carried out. GaAs Channel Figure 2.3: Cross-sectional transmission electron micrograph of a device structure with an annealed LTG-Alo.3 Gao.7 As passivation layer on top. Arsenic precipitates are seen as black dots in the micrograph. The AlAs diffusion barrier is shown to be effective in preventing the precipitates from diffusing into the device channel. An excess amount of As precipitates decorating the LTG-Alo.3 Gao.7 As/AlAs interface is also clearly shown [Courtesy o f J. P. Ibbetson]. 2.4.1 Basic Concept o f Experiment: Normally, in order to determine the channel bend-bending o f a heterostructure device, knowledge of the bulk Fermi level of each epitaxial layer (usually determined independently) along w ith the hetero-interface band offsets at all the relevance interfaces of the whole structure would be sufficient. However, in a heterogeneous material system such as that o f LTG-Alo.3 Gao.7 As, the bulk Fermi level is difficult to determine accurately, and the interface between the LTG layer to that of the normal epitaxial layer is still an unresolved question of the material properties. In this work, we have performed a direct electrical measurement of the channel band-bending. 22 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. A lA s t 5-doping GaAs Channel Figure 2.4: Schematic cross section of a 5-doping channel structure, with LTGAlGaAs passivation on top, used in the study of the interfacial properties of LTGAlGaAs to the normal channel. A possible corresponding band-diagram is shown on the right. The experiment makes use of a nominal 8 -doped channel structure shown in Figure 2.4. Typical epitaxial passivation layers of LTG-Alo.3 Gao.7 As were grown on top o f the active channel o f the device. An independent calibration of the 5-doping density was performed in a different experiment to ensure the accuracy of the correlation between the measured sheet charges and the channel band-bendings. Drawing from figure 2.4, the band-bending,d>, is directly proportional to the depleted charges in the channel, through the Poisson equation, ^ *1 ^ depleted tGaAs j tAlAs v. £ GaAs ^AlAs > where Ntdepleted is the total depleted sheet charge o f the channel and t are the respective thicknesses of the undoped layers. Using the above test structure, the effective channel band-bendings, with different LTG-Alo.3 Gao.7 As passivation layers, were deduced from the measured sheet charges via the Van der Pauw method. 23 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. 2.4.2 Effect o f Growth and Annealing Temperatures: Three samples with similar epistructures, except for the growth temperatures of the LTG-Alo.3 Gao.7 As passivation layers, have been studied. They were grown in an Intevac Gen II solid source MBE system. The structure consisted of a 5000A undoped GaAs buffer layer, then a Si 5-doped channel o f 1.4xl0 12 cm'2; followed by a 500A layer o f undoped GaAs, then 200A of AlAs and 25A o f GaAs. All these layers were grown at 590°C. The 25A o f GaAs was grown to prevent contamination during the cool-down and to present a clean surface for subsequent growth. Then, the substrate temperature was lowered to a predetermined temperature for the growth of the LTG layers. First, 25A layer o f LTG-GaAs was grown, and then followed by a 2000A layer o f LTG-Alo.3 Gao.7 As. The 25 A layer of LTG-GaAs was grown first to provide a smooth transition surface for the growth o f the LTG-Alo.3 Gao.7 As layer. The growth was finished with a 50A layer capping of LTG-GaAs on top of the whole structure. The growth procedure and parameters of the LTG-Alo.3 Gao.7 As passivation layers used in this experiment are designed to be identical to those used in the actual GaAs FET with LTG materials passivation, so that the data obtained from this experiment are o f direct relevance to the channel band-bending in the FET structures. Following growth, the wafers were cleaved into 6 x6 mm 2 samples. Annealings (ex-situ) o f these samples were performed in an AG & Associates Rapid Thermal Annealing (RTA) unit with flowing forming gas (90% N 2 and 10% H2) for 1 minute. A typical annealing ramp cycle is shown in figure 2.6. Table 2.1 tabulates the growth and annealing temperature conditions that have been investigated. After annealing, the samples were then processed for mesa isolation of the Van der Pauw pattern; and lastly ohmic contacts were deposited using e-beam evaporation. 24 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. Temp. Tanneal 300°C 30 sec | Time Figure 2.5: Annealing ramp-schedule of the LTG-Alo.3 Gao.7 As layers with flowing forming gas (90% N 2 and 1 0 % H2) ambient. Table 2.1: Summary o f the growth and annealing temperatures o f the LTGAlo.3 Gao.7 As layers studied. Tanneal is the highest temperature o f the annealing cycle shown in Figure 2.5 ^N^anneal 425 *C 450'C 475'C 500*C 525*C 550*C 575'C 600‘C 625’C 650*C tgrow tt^V 245*C 270’C 305’C X X X X X X X X X X X X X X X X X X X X X X The deduced effective channel band-bending (<I>) as a function o f growth and annealing temperatures from the measured Van der Pauw data are shown in figure 2.6. The annealing temperature range from 425°C to 650°C. The 425°C lower limit is a consequent o f the ohmic alloying temperature for the samples (which is typical in ohmic contacts for conventional GaAs devices); and the upper limit o f 650°C has been independently verified as the material limit where the AlAs layer still behaved reliably as an As diffusion barrier. A strong dependence of the channel band-bendings on both the growth and annealing temperatures is observed. Furthermore, this dependence is 25 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. also erratic, making it difficult to directly correate the interfacial property to that of the reported bulk material properties. Further studies are needed before conclusions about the nature o f the interface can be drawn. In addition, a set of control data obtained from a sample with the passivation layer selectively etched off are also shown in the figure. The channel band-bending o f the control data is shown to be relatively independent o f the annealing temperatures, this is could be view as an indication of the margin of error in our measurement.. 0 .9 £ os s I » 1 i » | 1 1 t "i r ‘| ■ 1 —^ ^ 0.8 i - r | - t ■!— r r ^ r « i - 1 i 1 capping layers removed ^ growth = 2 7 0 ’ C 0 .7 9i | n growth = 2 4 5 -C 0.6 "3 s c 0 .5 5 0 .4 growth = 3 0 5 -C as 0 .3 400 450 500 550 600 650 700 ^anneal ( ^ Figure 2.6: Deduced GaAs channel band-bendings due to growth and annealing temperatures o f the LTG-Alo.3 Gao.7 As layer. The dashed curve is from a sample with the LTG-Alo.3 Gao.7 As and AlAs layer selectively etched off by wet chemicals (sample Tgrowth =270°C). In comparison to LTG-GaAs, of which a plot o f the nominal Fermi level as a function of annealing temperatures is shown in figure 2.7, the behavior of the channel band-bending with LTG-Alo.3 Gao.7 As passivation as is markedly different. LTG26 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. Alo.3 Gao.7 As passivation resulted in channel band-bendings that are sensitively depended on the detailed growth and annealing temperatures. From a device engineering point o f view, these results indicated that different LTG-Alo.3 Gao.7 As materials passivation should have different impacts on device characteristics; in particular, parasitic resistances and low-frequency noise would be intimately influenced. 0.9 0.8 LTG-GaAs : Tgrowth= -200*C >V 0.6 0.4 0J 200 300 400 500 600 700 800 ^anneal 1 Figure 2.7: Typical Fermi level of bulk LTG-GaAs as a function of annealing temperatures [2 1 ]. At equilibrium, the channel band-bending is governed by the Fermi level o f the system at the interface between the LTG passivation layer and the rest of the channel. As illustrated in figure 2.3, and again on another sample grown at 270°C shown in figure 2.8, this annealed interface is decorated with a high density o f As precipitates. 27 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. Figure 2.8: Cross-sectional TEM of an LTG-Alo.3 Gao.7 As passivated sample grown at 270°C and annealed ex-situ using a RTA unit for I minute at 600°C. The interface of the LTG-AlojGaojAs-A lA s layer are shown to be decorated with excess As precipitates (similar to figure 2.3) [Courtesy o f J. P. Ibbeson]. However, the data shown in figure 2.6 for samples of different growth temperatures clearly do not converge to a single value for the channel band-bending (i.e., a single Fermi level). Taking into consideration the above channel band-bending data along with the cross-sectional transmission electron micrographs (figure 2 .3 and figure 2 .8 ), a picture that emerge from these data is that the precipitates alone are not sufficient to determine the Fermi level of the system, the point defects also played a very significant role. Using the condition o f charge neutrality, and nominal reported concentration o f deep donors and deep acceptors concentration (annealed LTGGaAs), it is seen that some o f the variation o f the Fermi level can be accounted for by the change o f concentration of defects as a function o f annealing temperatures (figure 2.9). However, although the calculation showed a plausible range of change in Fermi level, the magnitude is slightly off. This offset could be due to the uncertainty in the 28 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. energy levels o f these point defects. Further analysis to isolate the contribution from these precipitates and point defects required more detailed investigations (i.e., corresponding measurements o f the defect concentrations at the interface). This might not be possible, or very difficult to achieve; since this is an inherrent properties o f the LTG materials: the co-existence of both As precipitates and point defects in annealed LTG materials. 1.1 - Nrf = 1 x 10* 8 cm ' 0.9 uT ixj Cd 0.8 0.7 0.6 0.5 0 510‘ 7 1101 8 1.5 10* 8 210* Acceptor Concentration (cm' 3) Figure 2.9: Calculated values o f the Fermi level as a function of deep acceptors concentration (Ea= 0.3 eV from the valence band) using the condition of charge neutrality with the deep donors assumed to be 1x1018 cm *3 (Ed = 0.65 eV from the conduction band). 2.5 Summary : Established materials properties that are relevant to electronics devices were reviewed in this chapter. Materials science investigation in recent years have demonstrated that LTG-GaAs consist of a high concentration of point defects. The dominating active defects have been identified as AsGa and VQa, deep donors and deep acceptors, respectively. Furthermore, the concentrations of these defects have been demonstrated to be a strong function of both growth and annealing temperatures. 29 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. Further research are needed before a clear picture o f a correlation between the materials properties and processing parameters could be drawn. Meanwhile, the strong dependence o f the electrical properties on growth and annealing temperatures o f LTG-GaAs could readily be exploited to tailor the materials to yield desired property in their applications to device. Furthermore, emerging derivatives of LTGGaAs, such as LTG-Alo.3 Gao.7 As promised yet even better potentials for device engineering. Interfacial characteristics between the LTG-Alo.3 Gao.7 As passivation and the underlying normal GaAs channel has been systematically investigated. For device application, the data from Figure 2.6 provided a useful map of the parameter spaces for device designing with LTG-Alo.3 Gao.7As materials. Effective channel band bending of device can be readily inferred from the growth and annealing temperatures o f the LTG-Alo.3 Gao.7 As from this figure. 30 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. 2.6 References:  F. W. Smith, A. R. Calawa, C.-L. Chen, M. J. Manfra, and L. J. Mahoney, “N ew MBE buffer used to eliminate backgating in GaAs MESFETs,” IEEE Electron Device Letters, vol. 9, pp. 77-80, 1988.  L.-W. Yin, Y. Hwang, J. H. Lee, R. M. Kolbas, R. J. Trew, and U. K. Mishra, “Improved breakdown voltage in GaAs MESFETs utilizing surface layers of GaAs grown at a low temperature by MBE,” IEEE Electron Device Letters, vol. 11, pp. 561-563, 1990.  X. Liu, A. Prasad, W. M. Chen, A. Kurpiewski, A. Stoschek, Z. LilientalWeber, and E. R. Weber, “Mechanism responsible for the semi-insulating properties o f low-temperature-grown GaAs,” Applied Physics Letters, vol. 65. pp. 3002-3004, 1994.  M. Kaminska, E. R. Weber, Z. Liliental-Weber, R. Leon, and Z. U. Rek, “Stoichiometry-related defects in GaAs grown by molecular-beam epitaxy at low temperature,” Journal of Vacuum Science & Technology B (Microelectronics Processing and Phenomena), vol. 7, pp. 710-713, 1989.  M. Y. Kin, M. Kaminska, and Z. Liliental-Weber, “Characterization o f GaAs layers grown by low temperature molecular beam epitaxy using ion beam techniques,” Journal o f Applied Physics, vol. 72, pp. 2850-2856, 1992. [6 ] M. Kaminska, Z. Liliental-Weber, E. R. Weber, T. George, J. B. Kortright, F. W. Smith, B.-Y. Tsaur, and A. R. Calawa, “Structural properties o f As-rich GaAs grown by molecular beam epitaxy at low temperatures,” Applied Physics Letters, vol. 54, pp. 1881-1883, 1989.  M. Kaminska and E. R. Weber, “Defects in Semiconductors,” , G. Davies, G. G. DeLeo, and M. Stavola, Eds. Pennsylvania: Trans Tech, 1991. 31 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. [8 ] X. Liu, A. Prasad, J. Nishio, E. R. Weber, Z. Liliental-Weber, and W. Walukiewicz, “Native point defects in low-temperature-grown GaAs,’* Applied Physics Letters, vol. 67, pp. 279-281,1995.  D. C. Look, “Molecular beam epitaxial GaAs grown at low temperatures,” Thin Solid Films, vol. 231, pp. 61-73, 1993.  J. P. Ibbetson, J. S. Speck, N. X. Nguyen, A. C. Gossard, and U. K. Mishra. “The role o f microstructure in the electrical properties of GaAs grown at low temperature,” Journal o f Electronic Materials, vol. 22, pp. 1421-1424, 1993.  R. M. Feenstra, J. M. Woodall, and G. D. Pettit, “Observation o f bulk defects by scanning tunneling microscopy and spectroscopy: arsenic antisite defects in GaAs,” Physical Review Letters, vol. 71, pp. 1176-1179, 1993.  P. Kordos, A. Forster, J. Betko, M. Morvic, and J. Novak, “Semi-insulating GaAs layers grown by molecular-beam epitaxy,” Applied Physics Letters, vol. 67, pp. 983-5, 1995.  R. A. Metzger, T. Liu, W. E. Stanchina, R. G. Wilson, J. F. Jensen, L. G. McCray, M. W. Pierce, T. V. Kargodorian, Y. K. Allen, P. F. Lou, and U. K. Mishra, “Control o f Be diffusion in AlInAs/GalnAs heterostructure bipolar transistors through use o f low-temperature GalnAs,” Journal o f Vacuum Science & Technology B (Microelectronics Processing and Phenomena), vol. 10, pp. 859-862, 1992.  B. Elman, E. S. Koteles, P. Melman, K. Ostreicher, and C. Sung, “Low substrate temperature molecular beam epitaxial growth and the critical layer thickness o f InGaAs grown on GaAs,” Journal o f Applied Physics, vol. 70, pp. 2634-2640, 1991. 32 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission.  B. W. Liang, P. Z. Lee, D. W. Shih, and C. W. Tu, “Electrical properties of InP grown by gas-source molecular beam epitaxy at low temperature,” Applied Physics Letters, vol. 60, pp. 2104-2106, 1992.  W. M. Chen, P. Dreszer, A. Prasad, A. Kurpiewski, W. Walukiewicz, E. R. Weber, E. Sorman, B. Monemar, B. W. Liang, and C. W. Tu, “Origin o f n-type conductivity o f low-temperature grown InP,” Journal o f Applied Physics. vol. 76, pp. 600-602, 1994.  A. C. Campbell, G. E. Crook, T. J. Rogers, and B. G. Streetman, “Investigation of low growth temperature AlGaAs and GaAs using metalinsulator-semiconductor diagnostic structures.,” Journal o f Vacuum Science & Technology B (Microelectronics Processing and Phenomena), vol. 8 , pp. 305307, 1990.  Y. He, J. Ramdani, N. A. El-Masry, D. C. Look, and S. M. Bedair, “High resistivity LT-Ino.4 7 Gao.5 3 P grown by gas source molecular beam epitaxy." Journal o f Electronic Materials, vol. 22, pp. 1481-1485, 1993.  A. K. Verma, J. S. Smith, H. Fujioka, and E. R. Weber, “Characterization of low-temperature AlxGa[_xAs lattice properties using high resolution X-ray diffraction,” Journal o f Applied Physics, vol. 77, pp. 4452-4454, 1995.  L.-W. Yin, “GaAs Based Power Transistor Utilizing Low-Temperature GaAs Grown by MBE as the Surface Insulator,” : University of California, Santa Barbara, 1992.  J. P. Ibbetson, N. X. Nguyen, and U. K. Mishra, “AlAs and GalnP as diffusion barrier for GaAs surface layers grown at low temperature." presented at Electronic Materials Conference, Boulder, CO, 1994. 33 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. CHAPTER 3 Surface Layer Engineering to Improve Breakdown Voltage 3.1 Introduction: The surface plays a crucial role in the characteristics o f compound semiconductors devices, in particular high frequency devices. As o f present, the performance, uniformity, and therefore the cost of reliable microwave power FETs has been limited by the non-reproducibility o f the gate diode characteristics. The main reason for this is the lack of effective electrical passivation of the GaAs surface adjacent to the gate. In particular, the breakdown voltage of GaAs MESFET critically depends on the surface condition. Over the years, many efforts have been devoted into finding a viable solution to this fundamental problem. From a technological standpoint, the simplest solution for this problem would be to develop a controllable and reliable passivation technology for GaAs devices and materials. This is the approach that we have pursued over the course o f this project. An optimal passivation technology would be one that provides both environmental and electrical isolation of devices to external stimuli. As o f present. SiNx has been clearly demonstrated to be the most suitable environmental passivation layer in terms of preventing the change of the surface properties due to oxidation and humidity. It has been widely accepted by industry as the general environmental passivation layer for all electronic devices. However, an effective electrical passivation technology, on the other hand, has been much more elusive. To date, the most successful electrical passivation for the surfaces o f devices are those by chemical treatment. Photochemical oxidation and sulfide chemical passivation such as Na 2 S and (N R j^S [ 1 ], have been demonstrated to have the most 34 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. potential. However, these chemical treatments still leave devices susceptible to non uniformity and thermal instabilities. Furthermore, these technologies are inflexible to surface engineerings for device optimization. Therefore, an alternative, stable electrical passivation technology that is susceptible to surface engineering, is still very much sought after. As discussed in Chapter 2, the electrical properties o f LTG materials and their strong dependence on processing parameters, presented the materials as ideal candidates for the aforementioned sought after passivation technology. In this chapter, device surface engineering utilizing LTG passivation to improve breakdown voltage in GaAs MESFET is studied in detail. The first section of the chapter provides a synopsis of the problem of breakdown in GaAs power MESFET. Then the application o f LTG materials passivation to improve the breakdown voltage is presented and discussed. A physical model of the LTG material passivation, compensated deep donors (CDD) model, is proposed to explain the field redistribution obtained with passivated devices. This field redistribution would explain the experimentally observed improvement in the gate-drain breakdown voltage of LTG materials passivated FETs. A more quantitative study of the model has also been pursued. A full two dimensional electrostatic simulation and analysis of the device structures with LTG-GaAs passivation was performed. The results are presented and discussed. 3.2 Breakdown Voltage in GaAs Power MESFET: In general, breakdown in MESFETs occurs when the voltage supported by the depletion layer under the gate metal, and its associated electric field reach a critical limit of the material. When this happen, the resultant avalanche generation of 35 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. carriers by impact ionization leads to device failure. Analytically, avalanche breakdown is defined as the point when multiplication o f carriers in the depletion region by impact ionization rate reach infinity. Details o f avalanche breakdown physics can be readily found in many texts on semiconductor device physics . For a thick channel device, the depletion region extended downward into the channel, and the breakdown is essentially one dimensional, as shown schematically in figure 3.1a. The breakdown voltage could be analytically computed using Poisson’s equation and data from empirically measured critical field of the semiconductor channel involved. One dimensional breakdown voltage as a function of the doping concentration is shown in figure 3.1b. OURCE (a) WOOi 10: IMPURITY CONCENTRATION Ne (C n T 3 ) Figure 3.1: a) Schottky gate depletion of a thick channel FET structure - the depletion extended downward into the channel until breakdown occurs (i. e., when 36 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. the field at the metal-semiconductor reached the critical field strength), b) One dimensional avalanche breakdown voltage as a function of doping for an abrupt junction. However, for a thin channel structure, after reaching through the channel and into the buffer, the depletion region extends laterally toward the drain contact (shown schematically in figure 3.2). Therefore, the breakdown problem is two dimensional. The voltage that can be supported by such two dimensional depletion region is much higher than that of the one dimensional case, with values depending upon the thickness o f the channel. However this simplistic approach to improving the breakdown voltage of FETs is accompanied by a substantial reduction in the channel current density (thinner channel); thereby rendering the approach ineffective for high power devices. OURCE Figure 3.2: Gate depletion in a thin channel structure; the depletion region extends laterally toward the drain after pinching-off the channel - the field distribution is inherrently two dimensional. The compromising boundary, where the designed device would yield an optimized product o f the breakdown voltage and the channel current would resulted in a device structure with a maximum channel current density o f 400-450 raA/mm. With this design, the channel delivered the maximum possible current while retaining a two dimensional gate depletion characteristics. The breakdown voltage in such structure is very sensitive to the top surface boundary condition of the device. It is 37 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. the breakdown characteristics of this high-power device structure on which we have focused our research and development (figure 3.3). -V Figure 3.3: High power FET channel design where a compromise between the maximum drain current density and the breakdown voltage is achieved - the depletion region extends slightly toward the drain, and its exact characteristics depends sensitively on the top surface condition. 3.3 Breakdown Voltage Improvement by LTG Materials Passivation: The advent o f LTG materials and their unique properties presented an ideal solution to the aforementioned search for an ideal electrical passivation layer for GaAs devices and materials (discussed in Chapter 1). In effect, the LTG passivation layer presented a top surface boundary condition that can be engineered to deliver desired device characteristics. Indeed, experimental realization of MESFET with LTG-GaAs passivation were soon demonstrated. Subsequently, record breakdown voltage and power performance GaAs-based FETs were reported. But consistent reproducibility o f these results has been difficult due to the large parameter space of the LTG materials involved, and also a lack of clear understanding o f the exact mechanism that led to high breakdown voltage observed in passivated devices. It is generally hypothesized that the LTG-GaAs passivation acts as a charges absorber needed to alleviate the peak gate field . However, a physical model to explain this charge absorption mechanism of the LTG materials awaits further understanding and data from the materials science research. 38 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. Recent developments in material science o f LTG-GaAs have led us to believe that the compensated deep donor (CDD) o f the LTG material is the main cause of the observed improvement in the gate-drain breakdown voltage of the LTG-GaAs passivated FETs. Referring back to the discussion in Chapter 2 on electrical material properties o f LTG materials, there are two dominant and unique material properties o f LTG-GaAs that are critical to the effectiveness of this passivation technology. First, the materials contained a high concentration o f both type o f point defects, deep donors and deep acceptors, Asoa and Voa, respectively. Second, the deep donor concentration is always higher than that o f the deep acceptors. At equilibrium, the Fermi level of this material system is determined by the condition of charge neutrality: ne + N a = n h where ne = Ncexp[-(Ec - E f )/kT] nh = Nvexp[-(Ef - E v)/kT] and N~ = ---------------------------------- 1+ -exp[(E a - E f )/kT] g n; d = ------------ ^ ------------1+ gexp[(Ef - E d)/kT] A schematic band diagram of such a system is shown in figure 3.4. As illustrated in the figure, the deep acceptors are completely filled, but the deep donors are only partially filled. The density of empty donors, the compensated deep donors, is equal to the density of the deep acceptors in the system. In a device structure, these compensated deep donors provides the needed empty states for the absorption of negative charges being injected from the gate metal. In effect, they 39 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. plays a similar role to that o f the empty localized surface states reported by Barton e ta l[ 3]. F igure 3.4: Schematic band diagram of LTG-GaAs with both deep acceptors and deep donors, the compensated deep donors are shown as empty states above the Fermi level. Qualitatively, the compensated deep donors in the LTG passivation layer enables the layer to be effectively charged in the vicinity of the gate. This in turn leads to an alleviation of the peak field at the drain-end of the gate metal, thereby increasing the voltage that the device can accommodate before reaching the critical breakdown field. Mathematically, this is equivalent to a change o f the boundary conditions o f the electrostatic problem of the device; which can therefore dramatically alter the associated electric field distribution. Furthermore, a recent study by Ibbetson et al  has also demonstrated that the compensated deep donors led to a charge redistribution in the LTG-GaAs layer under high field. The study demonstrated that, at sufficient field strength, where the space-charged-limited transport is dominated, the CDD resulted in a development of extended space charges throughout the LTG materials. This phenomenon is schematically illustrated in figure 3.5. 40 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. (a) 7 = 0 NS-GaAs CE ef net space charge = 0 (b) J < J M Ef - — C ■r net space charge at interface (c) 7 > 7 p t, 1 z - extended space charge Figure 3.5: Space charge distribution in LTG-GaAs under applied field : a) in equilibrium, b) under low bias and c) under high bias. An extended space charge is developed throughout the LTG-GaAs layer under high field [From  ] It should be note here that the discrete trap levels nature o f this compensated deep donors model is a simplification o f the actual LTG materials properties; for there is recent evidence that the defect actually forms a band rather than discrete levels. Nevertheless, the general physics o f the field alleviation by empty states, provided by the compensated deep donors o f the model, would still remain valid. 3.4 Two Dimensional Electrostatic Simulation of LTG-GaAs Passivation: In order to confirm and to quantify the proposed model o f the breakdown voltage improvement in LTG passivated MESFET by compensated deep donors, a Ml two dimensional electrostatic analysis o f nominal device structures has been performed. A commercially available two-dimensional device simulation program, Silvaco’s BLAZE, was used for this purpose. However, due to the uncertainty in many physical parameters, such as mobility, saturation velocity, impact ionization 41 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. rate, and density and energy level o f the point defects in LTG-GaAs, no attempt was made to match the simulated device results to those obtained experimentally. The simulations are sought to provide further insights into the effect o f LTG-GaAs passivation rather than to quantify its effect on the device numerical figures-ofmerit. 3.4.1 Basic Semiconductor Equations: The Silvaco’s BLAZE program self-consistently solves a set of two dimensional equations. These equations governs the current-voltage distribution throughout the device structure. They are the Poisson equation, carriers current continuity equation, and drift-diffusion transport equation: divfsV'F) = -p where Poisson Equation is the electrostatic potential, £ is the permittivity, and p is the charge density. dn 1 j. - ^ ^ Current Continuity Equation where n and p are the electron and hole concentration, Jn and Jp are the electron and hole current densities, Gn and Gp are the generation rate for electrons and holes, Rn and Rp are the recombination rates for electrons and holes, and q is the magnitude of the charge on an electron. J n = n q itnE + qDnVn Driji-Diffusion Equation J p = pqM-pE - qDpVp Dn and Dp are the diffusion coefficients for electron and hole respectively; and the rest of the symbols are as defined above. 42 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. Carrier recombination via trap centers with a fixed lifetime is included in the simulation through the Shockley-Read-Hall model. Generation rates due to impact ionization are specified as : where = A n, p «exp V J The constants A and Ec are obtained experimentally for GaAs material : A=1.9xl0 5 cm'1, B=5.75xl0 5 V/cm, and m=1.82 for electrons; and A=2.22xl0 5 cm '1. B=6.57xl05 V/cm, and m=1.75 for holes. LTG-GaAs material was defined as normal GaAs with both deep donors and deep acceptors in the material. Various defect densities of (1-1.4) x 1018 cm*3 and (O.l-l) x 1018 cm' 3 were specified for donors and acceptors, respectively. These densities corresponds to the reported experimental data for annealed LTG-GaAs. 3.4.2 Simulation Results and Analysis: The cross-sectional structures of the MESFET used in the simulation are shown in figure 3.6. The channel composition and geometric dimensions for all device structures are the same, and they resembled the actual samples as much as possible. The channels are all 1500A thick, doped 3 x 1017 cm' 3 with silicon. Geometrically, a gate length of the simulated structure is 1pm, and the gate-source and gate-drain spacings o f 2 pm were used. For a control device, a structure with an undoped GaAs passivation layer, and a thin layer of top surface traps, density of lxlO 12 cm*2, for both deep donors and deep acceptors have been simulated. 43 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. ATLAS Dat a f r o m pit 1 a . s t r Materials M i c r o ns Figure 3.6: Cross section of device structures used in the two dimensional electrostatic simulations. The vertical dimension is the depth profile o f the device, and the lateral is the source/drain profile. Geometric dimensions are: 1 pm gate length, and 5 pm source-to-drain spacing. The channel is 1500 A o f n-GaAs doped 3xl0 17 cm*3. The compensated deep donors model of LTG-GaAs proposed in the previous section suggested that the two material parameters that would strongly affect the field alleviation mechanism of LTG-GaAs are the deep acceptors concentration and the energy level of the deep donors. In order to verify this hypothesis, simulations with different deep acceptor density (which is equivalent to the compensated deep donors density) were performed. A table o f the simulated parameters are summarized in Table 3.1. 44 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. Table 3.1: Summary o f trap parameters used in the device simulation. Ec -E d (eV) E a-E v (eV) Nd (cm*3) Na (cm*3) 1.0 x 1018 1.0 x 1017 0.7 03 1.0 x 10»8 3.0 x 1017 0.7 03 1.0 x 1018 5.0 x 1017 0.7 0.3 1.0 x 1018 7.0 x 1017 0.7 0.3 1.0 x 1018 9.0 x 10 17 0.7 03 1.2 x 1018 7.0 x 1017 0.7 0.3 1.4 x 1018 7.0 x 10 17 0.7 0.3 1.0 x 1018 7.0 x 10 17 0.5 0.3 l.Ox 1018 7.0 x 1017 0.3 0.3 Figure 3.7 shown a nominal potential distribution for two device structures, one is the control sample and the other is with simulated LTG-GaAs passivation (Nd = 1 x 10 18 cm-3 and Na = 7 x 1017 cm*3). The potential differences between gate to drain contacts for both structures were 15 V. In the control sample, the region of largest potential difference is clearly seen at the drain edge o f the gate metal, hence a peak electric field at that point. However, with simulated LTG-GaAs passivation, the electrostatic potential is shown to spread out over a longer distance, thus resulting in a lowered peak electric field at the same locale. 45 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. A'jftS D ctc fro m c " t'lc .s tr 025— 3oterl;d tv: Materials i « M 'c r o r s (a) AT.JVS D cta f'a r r . orL5 c .s t' 020- Polertioi (V) UoiericS M ic r o 's (h) Figure 3.7: Simulated two dimensional electrostatic potential distribution with a) undoped GaAs passivation; b) LTG-GaAs passivation (defined with Nd = lxl 0 18 cm’3 and Na = 7x10 17 cm*3). 46 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. Systematic simulations of the gate-drain breakdown voltage dependence on the deep acceptors are shown in Figure 3.8. As expected from the compensated deep donor model, the breakdown voltage is a strong function o f the deep acceptors density. An improvement o f over 75% (12V versus 6 .8 V) in term o f breakdown voltage is observed in figure 3.8. Furthermore, in order to verify that it is the empty states of the compensated deep donors that play the central role in field alleviation and not the total deep donors concentration, a simulation where the deep acceptors concentration were fixed while the deep donors concentration varied were performed. A few selected breakdown voltages as a function o f the total deep donors concentration are shown in figure 3.9. The curves showed the breakdown voltages dependence on the total deep donors concentration to be negligible. 0.010 * ^Control N. =9x1017cm • 1.0 10 •16 -14 -12 ■6 •10 -4 -2 0 Gate-Drain Voltage (V) Figure 3.8: Breakdown voltage as a function of deep acceptor concentration of LTG-GaAs. The control sample is defined as having undoped GaAs passivation with j ust surface traps (Na= 1 x 1 0 12 cm *2 and Nd= 1 x 1 0 12 cm*2) 47 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. 1.010 - 1.0 10 S - 2.0 10 c - 3 .0 10 u<. - 4 .0 1 0 S w 3 N . = 1 .0 x 1 0 cm N . = 1 .4 x 1 0 * c m - 5 .0 10 - 7 .0 10 -1 6 •14 -12 •8 -10 ■6 0 V o l t a g e (V ) Figure 3.9 : Breakdown voltage dependence on deep donnor concentration of LTGGaAs. Other parameters o f the simulated LTG-GaAs are shown in the inset. In addition to trap concentrations, the breakdown voltage dependence on the deep donor energy levels were also performed. The effect of the donor levels on breakdown voltages is shown in figure 3.10. For the same concentration o f defects in LTG-GaAs, it is seen that the deep donor level at 0.7 eV resulted in an optimal breakdown voltage. Qualitatively, this observation can be explain by the efficiency of the capturing and emission of electrons by the traps; in addition, it is also consistent with our proposed model of CDD. The deep donor level at midgap (0.7 eV) would result in the maximum capture time o f the electrons (i.e. maxium retention of electrons) by the CDD traps, hence making the alleviation of the peak field by the LTG passivation most efficience. As this electron trap level gets shallower, re emission o f electrons from the trap increased, thereby drastically reducing the field alleviation efficency o f the LTG layer. 48 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. 0.0 10 ° '0.7 eV ^■E -E . =‘0.5 eV 1 -4 .0 10’s 4 .0 1 0 -16 -14 -12 •10 -8 -6 •4 -2 0 Voltage (V) Figure 10: Breakdown characteristics versus deep donor energy levels in simulated LTG-GaAs. The lowest breakdown is achieved with the donor at midgap. The concentrations and deep acceptor energy levels are indicated in the inset. 3.5 Sum m ary : The present chapter focuses on the physics o f the breakdown voltage in GaAs microwave power FETs. In an optimally designed FET structure for high output power, the electrostatic distribution o f the device is inherrently two dimensional. Furthermore, this electrostatic distribution depended sensitively on the boundary conditions o f the structure. In term o f device engineering, these dependences meant that the breakdown voltage of a FET structure is very sensitive to its surface conditions. Consequently, the proper engineering of the surface passivation layer, or equivalently the boundary condition, could lead to dramatic improvement in the breakdown voltage of devices. Experimentally, improved breakdown voltages in GaAs FET have been demonstrated through various geometrical surface engineering techniques [5-7]. 49 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. Recently, empirical surface engineering with LTG-GaAs and its related materials passivation in GaAs [8 - 10 ] had also been demonstrated to dramatically improve the device breakdown voltages in GaAs FETs. However, the exact physical mechanism that lead to this improvement of gate-drain breakdown voltage was unclear. Drawing from recent advances in the understanding o f material sciences of LTG-GaAs, we are proposing that the compensated deep donors is the main attribute in the LTG-GaAs passivation that enabled it to improve the breakdown voltage when utilized in a FET structure. A full two dimensional electrostatic simulation o f the effect of LTG-GaAs passivation in FETs using the proposed model o f compensated deep donors have been performed. Although the two discrete trap levels used in the model is an oversimplification of the actual traps in LTG materials, the physics of the problem should remain the same. The breakdown voltage in the structure is observed to be strongly dependent upon the compensated deep donors concentration. Futhermore, it is also sensitively depended on the energy level o f the donor trap. These strong dependencies would explain the low reproducibility observed in LTG-GaAs passivated devices; this is a consequent of the fact that both the trap densities and energy levels in LTG materials have been reported to be a strong function of both growth and annealing temperatures [II, 12 ]. However, these dependencies are also indications that the LTG materials passivation would be suitable for material engineerings to obtain high breakdown voltage in devices. 50 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. 3.6 References:  E. Yablonovitch, B. J. Skromme, R. Bhat, J. P. Harbison, and T. J. Gmitter, “Band bending, Fermi level pinning, and surface fixed charge on chemically prepared GaAs surfaces,” Applied Physics Letters, vol. 54, pp. 555-557, 1989.  C.-L. Chen, “Breakdown of overlapping-gate GaAs MESFETs,” IEEE Transactions on Electron Devices, vol. 43, pp. 535-542, 1996.  T. M. Barton, “Simulation of surface state dynamics on GaAs MESFETs,” European Transactions on Telecommunications and Related Technologies, vol. l,pp. 393-400, 1990.  J. P. Ibbetson and U. K. Mishra, “Space-charge-limited currents in nonstoichiometric GaAs,” Applied Physics Letter, vol. 68, pp. 3781-3783, 1996.  S. H. Wemple, W. C. Niehaus, H. M. Cox, J. V. Dilorenzo, and W. O. Schlosser, “Control o f gate-drain avalanche in GaAs MESFETs,” IEEE Transactions on Electron Devices, vol. 27, pp. 1013-1018, 1980. [6 ] T. Furutsuka, T. Tsuji, and F. Hasegawa, “Improvement of the drain breakdown voltage of GaAs power MESFETs by a simple recess structure,” IEEE Transactions on Electron Devices, vol. 25, pp. 563-567,1978.  T. Furutsuka, A. Higashisaka, Y. Aono, Y. Takayama, and F. Hasegawa, “GaAs power MESFETs with a graded recess structure,” Electronics Letters, vol. 15, pp. 417-418, 1979. [8 ] L.-W. Yin, Y. Hwang, J. H. Lee, R. M. Kolbas, R. J. Trew, and U. K. Mishra, “Improved breakdown voltage in GaAs MESFETs utilizing surface 51 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. layers o f GaAs grown at a low temperature by MBE,” IEEE Electron Device Letters, vol. 11, pp. 561-563, 1990.  C.-L. Chen, L. J. Mahoney, M. J. Manfra, F. W. Smith, D. H. Temme, and A. R. Calawa, “High-breakdown-voltage MESFET with a low-temperaturegrown GaAs passivation layer and overlapping gate structure,” IEEE Electron Device Letters, vol. 13, pp. 335-337, 1992.  N. X. Nguyen, J. P. Ibbetson, J. C. Yen, M. H. Hashemi, and U. K. Mishra, “Encapsulated GaAs power MESFET.,” Proceedings. IEEE/Cornell Conference on Advanced Concepts in High Speed Semiconductor Devices and Circuits (Cat. No.93CH3235-9), pp. 539-47, 1993.  X. Liu, A. Prasad, W. M. Chen, A. Kurpiewski, A. Stoschek, Z. LilientalWeber, and E. R. Weber, “Mechanism responsible for the semi-insulating properties o f low-temperature-grown GaAs,” Applied Physics Letters, vol. 65, pp. 3002-3004, 1994.  M. Kaminska, E. R. Weber, Z. Liliental-Weber, R. Leon, and Z. U. Rek, “Stoichiometry-related defects in GaAs grown by molecular-beam epitaxy at low temperature,” Journal o f Vacuum Science & Technology (Microelectronics Processing and Phenomena), vol. 7, pp. 710-713, 1989. 52 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. B CHAPTER 4 Experimental Implementation o f LTG-AlGaAs Passivation 4.1 Introduction: The two dimensional electrostatic simulations from Chapter 3 have clearly confirmed the strong correlation between the gate-drain breakdown voltage o f passivated GaAs MESFET, and the defects concentrations in its LTG passivation layer, especially the deep acceptor concentrations. These defects concentrations, in turn, are sensitively dependent upon the synthesis processes, such as, the growth temperature and the subsequent thermal treatment of the LTG materials. Preliminary device results first reported by Chen et a l[ 1], and also independently by Yin et al [2, 3] in 1992, provided clear experimental demonstration of the feasibility of the LTG material passivation technology. However, in those early works on LTG-GaAs passivated GaAs MESFET, only one growth and annealing condition was investigated. Namely, the LTG-GaAs passivation layer was grown at ~200°C and annealed in-situ at 600°C for 10 minutes under arsenic over pressure. Other growth and annealing temperatures, which have been demonstrated to yield unique LTG material properties  have not been in investigated in devices. Therefore, from a device engineering point o f view, a systematic study of the dependence of the device characteristics on both the growth and annealing temperatures o f the LTG passivation layer was called forth. This study would yield imperative informations in determining the suitability of this technology for widespread applications. Such study is the subject of the present chapter. In this study, the LTG-Alo.3 Gao.7 As surface passivation for GaAs power MESFET have been investigated in details. 53 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. As discussed in section 2.3, LTG-Alo.3 Gao.7 As shares many similar properties to those of LTG-GaAs, but with a larger bandgap; thus, the critical breakdown field o f LTG-AIo.3 Gao.7 As should be higher, and the leakage current in LTG-Alo.3 Gao.7 As passivated devices should also be lower. The gate field alleviation mechanism provided by the compensated deep acceptors in LTG materials should also be applicable to LTG-Alo.3 Gao.7 As passivation. A combination o f these two properties made LTG-Alo.3 Gao.7 As passivation a naturally preferred material for high power devices. The first section o f the chapter, following the introduction, describes the device design and fabrication that we have undertaken to experimentally study the effect o f growth and annealing temperatures on the gate-drain breakdown voltage. Device results and analysis are presented in the followed section. The impact of the growth and annealing temperatures o f the passivation layers on device characteristics such as, current voltage relationships and in particular the gate-drain diode characteristics are presented and discussed. In addition, a preliminary study o f the effect of the LTG-Alo.3 Gao.7 As passivation parameters on the low-frequency noise characteristics of the devices are also presented. Lastly, a summary o f the main findings from the present investigation is given. 4.2 Device Design and Fabrication: As evidenced in the literature on GaAs power MESFETs [5-7] and also from our independent data [8 ], the breakdown voltage of a MESFET is found to be very sensitive to its exact surface condition, which in turn depends strongly on the fabrication steps that the device. Systematic measurements o f the gate-drain breakdown voltage in conventional GaAs MESFETs across a sample have been shown to varied by over 50% . This large margin of experimental errors, although 54 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. typical in standard MESFET fabrication, has made the investigation of the cause of breakdown voltage in GaAs MESFET a daunting one. In particular, it made the systematic study o f new techniques for improving breakdown voltage, such as LTG materials passivation, difficult. The task of isolating the effects that arise from the LTG-Alo.3 Gao.7As passivation, and those that are due to processing variations has proved to be non-trivial. In order to overcome this experimental obstacle, we have designed a device fabrication process that allowed us to minimize the impact o f the processing variation on the data, therefore single out the effects of LTG-Alo.3 Gao.7 As material parameters on the device characteristics. We started with an epitaxial growth of a typical MESFET structure: 5000A o f undoped GaAs buffer, then 1500A of n-GaAs channel with Silicon doping of 3.5x10 17 cm-3, and then capped with a 400A InxG ai-xAs graded contact layer doped to 1x1019 cm*3. After the growth o f the wafer, a refractory metal, Tungsten (W), was used to defined the source and drain contacts. The wafer was then sectored and each piece was separately reload for the regrowth o f the LTGAl0 3Ga<) 7A s passivation layer. The samples were loaded into an in-situ etch chamber. Chemical gas etching (CGE) with chlorine was then used to etch away the grading contact layer. A laser monitor was used for process control of the etch depth. Following the etch, each sample was transferred to an Molecular Beam Epitaxial (MBE) chamber for the regrowth of the LTG-Alo.3 Gao.7 As passivation layer. The transferring process between the etching chamber and the MBE chamber was done under ultra-high vacuum to protect the surface o f the samples from potential surface contamination and oxidation. The regrowth started with an AlAs barrier layer followed by a non-stoichiometric AlGaAs layer, with growth temperature as the discriminating parameter between the samples. 55 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. G ra d e d C o n ta c t L aver Growth of epitaxial structure with grading non-alloyed contact layer. n -G a A s C hannel S I G aA s raided C o n ta c t L ay er Tungsten (W) sputtering to define source/drain n -G a A s C hannel S I G aA s In-situ etching of contact layer with CI2 chemical gas etching (CGE) n-GaAs Channel SI GaAs LTG-AIGaAss Blanket regrowth of LTG materials on etched sample n -G a A s C h ann el S I G aA s Mesa isolation etching with CI2 reative ion etching (RIE) Selective etching of LTG materials in gate region with CI2 (RIE) n -G a A s C h ann el SI G aA s Tungsten (W) gate metallization n -G a A s C hannel S I G aA s Figure 4.1: Flow chart o f an all-refractory metals MESFET fabrication process; the corresponding device cross sections are shown on the right. Following the regrowth of the passivation layer, the samples were unloaded and processing o f the devices continued. Device mesa isolation was defined by 56 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. chlorine reactive ion etching (CI2 RIE). The polycrystalline overgrowth over the W contacts was selectively etched using Cl2 RIE. The fabrication process was then finished with the recess etching o f the LTG-Alo.3 Gao.7 As in the gate region, followed by a gate metallization with W sputtering. A flow chart o f the process and the corresponding device cross-section is shown in Figure 4.1. This process provided FETs on identical channel material, with epitaxial passivation grown at various temperatures, ready to be monitored as a functions of annealing temperature. The refractory nature o f both the Schottky gate and the non-alloyed ohmic contacts enable them to be relatively independent o f the subsequent annealing treatment and allowed us to monitor just the effects o f annealing of the LTG-Alo.3 Gao.7As passivation layer on device characteristics Utilizing the fabrication process described above, we have prepared samples with different growth temperatures o f the LTG-Alo.3 Gao.7 As passivation layer. The growth and annealing parameter space that were investigated are summarized in Table 4.1. The annealing cycle is similar that detailed in Section 2.4. Table 4.1: Summary o f growth and annealing temperatures investigated. ^^anneal 245‘C 270'C 305‘C 350’C none 300*C 400*C 500*C 550*C 575*C 600’C X X X X X X X X X X X X X X X X X X X X X X X X X X X X 57 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. 4.3 Device Results and Analysis: 4.3.1 Characteristics o f Devices with Unannealed LTG-AlojGao, 7As Passivation Figure 4.2 shows the room temperature gate-drain diode characteristics of unannealed devices with different LTG-Alo.3 Gao.7 As growth temperatures. The gatelength of the devices is 1.2pm, and the width is 300pm. The source to drain spacing is 5pm. The control device, where normal undoped GaAs passivation material was grown, had a breakdown voltage o f 9V (typical for GaAs MESFET channel with similar doping density ). The devices with LTG-Alo.3 Gao.7 As passivations show dramatic improvement in the breakdown voltage. 0.5 c <u uu S U growth = 245 'C 43 u -0 . 5 Control = 270 -50 -40 growth = 350 *C "C -30 -20 -10 0 Gate-Drain Voltage (V) Figure 4.2: Experimental data o f MESFET gate-drain breakdown voltage as a 58 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. function of growth temperatures o f the LTG-Alo.3 Gao.7As passivation layer. The gate length of the device is 1 .2 pm, and the source to drain spacing is 5 pm. 4.3.2 Effect o f Annealing on Gate-Drain Breakdown Voltage A typical current-voltage characteristic is shown in figure 4.3. The full channel currents o f the various FETs were similar and therefore the comparison of the breakdown voltages is relevant. Figure 4.4 shows the breakdown voltages of the various FETs as function of anneal temperature. Also shown is the variation of the breakdown voltage of the control sample, as a function of anneal temperature, where the epitaxial passivant was an undoped GaAs layer grown at normal temperature of 600'" C. This could, in a sense, be an indication o f the margin of error in our measurements. Breakdown voltage was defined as the voltage at which the gate-drain diode leakage was 1 mA/mm. The main feature of the breakdown voltage dependence on the preparation conditions o f the LTG-Alo.3Gao.7As passivation layer is the relatively monotonic decrease o f the breakdown voltage with anneal temperature, independent of the growth temperature to a temperature o f ~550°C. Then, in most samples, there is a precipitous drop in the breakdown voltage over a narrow range of temperature, down to the low breakdown voltage o f the control sample. There are two possible reasons for this decrease. Either the concentration o f the empty donors (equal in concentration to the filled acceptors assumed to be the Ga vacancy) reduces to below levels which are effective (i.e. ~2-3 x 1017 cm'3) or the spreading o f the electric field due to the surface resistor formed by hopping conduction is impeded. The dilemma we currently 59 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. face is that if electron injection into the hopping band is at all possible (necessary- for both mechanisms) then hopping conduction has to occur. The absolute magnitude of 500 40 0 £ E < 300 E s <u u u 2 00 3 u 100 0 1 2 3 4 5 Drain Voltage (V) Figure 4.3: Typical current-voltage characteristics o f GaAs MESFETs with regrown LTG-Alo.3 Gao.7As passivation. Gate voltage started from IV, with a step o f -1 V. the hopping conductivity is not important since, at DC, the voltage drop is always linear, independent o f the resistivity. Hence redistribution of the field should be effective even after a 600°C anneal. This experimentally does not happen as evidenced by the collapse o f the breakdown voltage in figure 4.4. The major exception is the sample grown at 245°C, the sample with the highest degree of non-stoichiometry. The data seem to suggest the following scenario. Annealing the device above 500°C to 550°C leads to the elimination of hopping conduction in the thin (2 0 0 0 A thick) LTG-Alo.3 Gao.7As passivation layer between the gate and the drain. This can 60 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. only happen if the donor density in this surface oriented film decreases substantially faster than in the bulk films on which transport measurements were normally carried out  or by a disconnection between the metal and the hopping band. The first can occur by a diffusion o f defects laterally to the gate metal, depleting the donor density proximal to the metal thereby increasing the tunneling distance into and effectively disconnecting the hopping band. The sample grown at 245°C does not show the variation with anneal temperature could be simply related to a large enough donor density in the film to survive the issues mentioned above. 50 > 40 v ea 33 o 30 C £ o ■ ■C 3oC 3 20 s as-grown BV defined as Ig = 1 mA/mm co 10 i - 200 ..I i . i . L 250 i Control (BV=8.5 V) i i i _ i _ i_ i t _ i i 300 350 Growth Temperature j— l — i - i 400 (a) 61 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. 50 Tgrowth = 270°C 40 Tgrowth = 305°C o 00 93 o > 30 Tgrowth = 350°C c ? To3 IS V w. ca Tgrowth = 245°C 20 10 Control 0 250 300 350 400 450 500 550 Annealing Temperatures (°C) 600 650 (b) Figure 4.4: Breakdown voltage as a function of growth temperature and anneal temperature of LTG-AlGaAs cap (a) as-grown and (b) annealed ex-situ using an RTA system. 4.3.3 Effect o f Annealing on Low-Frequency Noise In addition to influencing the gate-drain breakdown voltage, LTG materials passivation has been shown to dramatically affect the low-frequency noise characteristics o f the passivated devices. We systematically investigated the effect of the preparation conditions o f the LTG-Alo.3Gao.7As passivation on the low frequency noise of FETs with a gate length of 1 pm. The control sample was the same as that discussed in the earlier section; had undoped GaAs as a passivant. Figure 4.5 and 4.6 display the low frequency noise characteristics obtained for annealing temperatures, 62 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. o f 500°C and 550'C. respectively for devices with various growth temperatures. As can be seen readily, LTG-Alo.3Gao.7As passivated devices consistently displayed better lower low-frequency noise than that of the control device. -70 Tanneal = 500*C •80 -90 — -100 ea -110 Control Tg = 305*C -130 Tg = 270'C -140 Tg = 35(f C -150 t 1 10 100 1000 10000 100000 1000000 Frequency (Hz) Figure 4.5: Low-frequency noise spectrum of GaAs MESFETs with LTGAl0 3 Gao 7As passivation grown at temperatures indicated in figure and annealed at 500°C. As can be seen in figure 4.5, for the annealing temperature o f 500°C, the best low frequency noise are obtained for the samples with passivation grown at 245°C and 350°C. The sample with LTG-Alo.3Gao.7As passivation grown at 245°C showed a comer frequency o f 30 kHz, much lowered than the typical 1 MHz comer frequency reported in GaAs MESFET . (Caution is in order here - A true comer frequency can only be defined if the white noise floor of the device is unequivocally established. 63 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. -70 Tanneal = 550’C -80 -90 -=• -100 s -110 Control Tg = 245”( Tg = 270‘C Tg = 305*C Tg = 350*C -130 -140 -150 1 10 100 1000 10000 100000 1000000 Frequency (Hz) Figure 4.6: Low-frequency noise spectrum of GaAs MESFETs with LTGAlo.3Gao.7As passivation grown at various temperatures and annealed at 550°C . This has not been done in a definitive sense in this case and hence we emphasize the low magnitude o f the low frequency noise across the spectrum rather than a comer frequency). However, when annealed at 550°C, the low-frequency noise o f the LTGAlo.3 Gao.7As (245°C) increased while that of the LTG-Alo.3Gao.7As (305°C) remained essentially the same. Upon annealing at yet higher temperature, 575°C, the lowfrequency noise o f the LTG-Alo.3Gao.7As (245°C) recovered the value close to that of the one annealing at 500°C (figure 4.7). 64 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. -90 Tgrowth = 245'C -100 -110 > Ta = 550'C -120 Ta = 575*C £ -130 Ta=500*C -140 -150 1 10 100 1000 10000 Frequency (Hz) 100000 1000000 Figure 4.7: Low-frequency noise spectrum o f a GaAs MESFET with LTGpassivation, grown at 245°C and annealed at temperatures indicated in the figure. A lo .3 G a o 7A s The understanding of 1/f noise in a surface oriented device such as a FET is extremely difficult. It has been empirically established,  and references therein, (with supporting theories presented) that the surface of the FET is a major source o f the low-frequency noise. A single trap with a well defined energy provides a generation-recombination (G-R) center and can lead to excess noise at frequencies close to the resonance frequency of the trap and produce a G-R bulge superimposed on the l/f noise spectrum, but, cannot produce the entire spectrum. Such G-R bulges are common and a classic case is that produced by the DX center in AlGaAs-GaAs HEMTs. A trap-based model for the observed l / f noise requires a spectrum of energy states. The surface of a FET provides such a continuum o f states. The model in its essence is that charge fluctuations at the device surface cause conductivity 65 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. fluctuations in the channel which in turn lead to l/f noise. If that is so then screening the surface effectively should suppress the low-frequency noise. This requires an epitaxial layer with mobile charges which can respond in the time constant typical of the spectrum (lp s) to screen the surface potential fluctuations. This layer should not have detrimental consequences such as high gate leakage and lower breakdown. This requirement seems to be best met by an epitaxial layer with a deep donor hopping band, the very properties of LTG epitaxial layers. A model that we believed would qualitatively explain the low-frequency noise suppression in LTG passivated devices is detailed below and shown schematically in figure 4.8. A deep donor hopping band at 0.4 eV and an anti-site band at a nominal 0.7 eV is shown. Our model requires charge exchange between the hopping band and the surface so that effective screening can occur. Charge exchange is only possible between bodies with a work function difference. Therefore, the work function o f the LTG-epitaxial layer should be smaller than that o f the surface i.e. <0.7 eV. Also for screening to effectively occur the hopping band has to be able to communicate with the gate metal and the contact. This requires thermionic field emission to be from the gate metal to the adjacent hopping band. This indicates that the l/f noise elimination will be determined by the relative magnitude o f hopping density of states and the tunneling probability from the gate metal. The required conditions are most effectively achieved with two donor bands (which seem to occur readily in LTG GaAs). Both of these are a function o f preparation conditions and is reflected in the data. 66 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. □lain N -Sepitaxial la y e r n epitaxial layer T A- A.*------------------------------- Figure 4.8 : Screening of surface potential fluctuations by hopping band of the LTG materials. 4.4 Sum m ary: The present chapter presented a thermally stable device fabrication process that is well suited for the study o f the LTG materials passivation technology. Devices fabricated using this process allowed us to systematically study the effect of growth and annealing temperatures on the device characteristics. This study in turn clearly demonstrated the potential o f the LTG-Alo.3 Gao.7 As passivation as a potential electrical passivation technology for GaAs devices and circuits. By engineering the LTG-Alo.3 Gao.7 As material properties through its synthetic process, device characteristics could be dramatically impacted. Very high gate-drain breakdown voltage, and also ultra low low-frequency noise have been experimentally demonstrated. Furthermore, the temperature dependence o f the breakdown on the growth temperature of the LTG-Alo.3 Gao.7 As layer provided strong supporting evidences for the model o f field alleviation by the compensated deep donors of LTG materials proposed in Chapter 3. 67 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. 4.5 References :  C.-L. Chen, L. J. Mahoney, M. J. Manfra, F. W. Smith, D. H. Temme, and A. R. Calawa, “High-breakdown-voltage MESFET with a low-temperaturegrown GaAs passivation layer and overlapping gate structure,” IEEE Electron Device Letters, Vol. 13, pp. 335-337, 1992.  L.-W. Yin, “GaAs Based Power Transistor Utilizing Low-Temperature GaAs Grown by MBE as the Surface Insulator,” : University o f California, Santa Barbara, 1992.  L.-W. Yin, N. X. Nguyen, K. Kiziloglu, J. P. Ibbetson, A. C. Gossard, and U. K. Mishra, “Device performance of submicrometre MESFETs with LTG passivation,” Electronics Letters, Vol. 29, pp. 1550-1551, 1993.  P. Kordos, A. Forster, J. Betko, M. Morvic, and J. Novak, “Semi-insulating GaAs layers grown by molecular-beam epitaxy,” Applied Physics Letters, Vol. 67, pp. 983-5, 1995.  T. M. Barton and P. H. Ladbrooke, “The role of the device surface in the high voltage behaviour o f the GaAs MESFET,” Solid-State Electronics, Vol. 29, pp. 807-813,1986. [6 ] W. R. Frensley, “Power-limiting breakdown effects in GaAs MESFETs,” IEEE Transactions on Electron Devices, Vol. 28, pp. 962-970, 1981.  H. Mizuta, K. Yamaguchi, and S. Takahashi, “Surface potential effect on gatedrain avalanche breakdown in GaAs MESFET's,” IEEE Transactions on Electron Devices, Vol. 34, pp. 2027-2033,1987. [8 ] N. X. Nguyen, J. P. Ibbetson, J. C. Yen, M. H. Hashemi, and U. K. Mishra, “Encapsulated GaAs power MESFET.,” Proceedings. IEEE/Cornell 68 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. Conference on Advanced Concepts in High Speed Semiconductor Devices and Circuits (Cat. No.93CH3235-9), pp. 539-47, 1993.  S. H. Wemple, W. C. Niehaus, H. M. Cox, J. V. Dilorenzo, and W. 0 . Schlosser, “Control o f gate-drain avalanche in GaAs MESFETs,” IEEE Transactions on Electron Devices, Vol. 27, pp. 1013-1018, 1980.  Y. Aokie and Y. Hirano, High-power GaAs FETs. Boston London: Artech House Inc., 1993.  J. P. Ibbetson and U. K. Mishra, “Space-charge-limited currents in nonstoichiometric GaAs,” Applied Physics Letter, Vol. 68, pp. 3781-3783, 1996.  B. Hughes, N. Fernandez, and J. Gladstone, “GaAs FETs with a flicker-noise comer below 1MHz,” IEEE Transactions on Electron Devices, Vol. 34, pp. 733-741, 1987.  A. D. van Rheenen, Y. Lin, S. Tehrani, C.-L. Chen, and F. W. Smith, “Noise studied o f HFETs on low temperature grown GaAs buffers and o f MESFETs with low temperature grown GaAs passivation,” Materials Science & Engineering B (Solid-State Materials fo r Advanced Technology), Vol. B22, pp. 82-85, 1993. 69 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. CHAPTERS High Performance GaAs Microwave Power FET 5.1 Introduction: The ultimate manifestation o f all device engineering with LTG materials passivation to improve breakdown voltage is in the power performance o f the device . The power performance is of paramount importance because no matter how much we have leamt about the effects of LTG-Alo.3 Gao.7 As passivation on device, the engineering bottom line remains whether or not the LTG passivated device would be up to expectation when they are used in microwave circuits. For circuit applications, the device power figures-of-merit that mattered are: output power density, power-added-efficiency, linear gain, and intermodulation distortion [2 . 3], These figures-of-merit provides the truest testimonies o f the suitability o f the LTG passivation technology for microwave power devices. The next section o f this chapter focused on the device design and fabrication of a power field effect transistor which utilized the LTG-Alo.3 Gao.7 As passivation technology for improved gate-drain breakdown voltage. Then followed by a section on device results and analysis. DC and RF characteristics of the device is presented and discussed, and then the continuous-wave on-wafer power performance of the device are presented. Finally, a summary of the main points of the chapter is given. 5.2 Device Design and Fabrication: In order to optimize channel design for high power, a doped channel heterostructure field effect transistor is used . The device epitaxial structure was grown using a Varian Gen II MBE system on semi-insulating LEC GaAs substrate. First, a buffer layer o f 5000A GaAs was grown at a substrate temperature o f 600"C. 70 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. followed by a 300A o f undoped Alo.3 Gao.7 As charge confinement barrier, then a 1000A layer of n-GaAs channel doped with Silicon at Nd = 3x10 17cm -3 was grown, followed by another 300A layer of Alo.3 Gao.7 As. Next, an arsenic-diffiision-barrier of 200A o f AlAs was grown, which was capped with a 50A layer o f GaAs. The substrate temperature was then lowered to 200°C, where 2000A o f LTGAlo.3 Gao.7 As was grown. The sample was then annealed in-situ with As over pressure at 600°C for 10 minutes. A sample with a similar epitaxial structure but with the replacement o f the LTG-Alo.3 Gao.7 As passivation layer by an undoped normal temperature grown Alo.3 Gao.7 As was also grown as a control. A schematic cross section of the structure is shown in Figure 5.1. ' 50XXTG-C»As ^growth = 245 C 200A AlAs 50A GaAs "7ooX"AIgjGaJJ^A!r" 50A Spacer 10004 3x1017 cm-3 GaAs } 50A Spacer 3 0 0 A. A I q j G i q j A s Si 5-doping 1x1012 cm-2 ^growth 5 590 C 5000 A GaAs Buffer Sem i-Insulating GaAs Substrate Figure 5.1: Schematic cross section o f a high-power GaAs heterostructure field effect transistor (HFET) with LTG-Alo.3 Gao.7 As passivation incorporated to improve breakdown voltage. Room temperature Van der Pauw measurement o f an actual sample yield a sheet charge of 5x10 12 cm *2 and a mobility of 3650 cm 2 /V-s. Processing began with the selective regrowth of the source/drain contacts with n ^ -G a A s by Metal Organic Chemical Vapor Deposition (MOCVD) , Followed by e-beam evaporation of AuGe/Ni/Au metals. The selective regrowth was 71 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. accomplished at 550°C, well below the in-situ annealing temperature o f the LTGAlo.3 Gao.7 As layer. Inter-device isolation was achieved by boron ion implantation. Next, a 1.2 pm long gate foot print was defined using photolithography; then Cb reactive-ion-etching was used to etch away the LTG-Alo.3 Gao.7 As and expose the channel. Finally, a 2 pm overlapping gate mask was aligned to the defined gate foot print and the gate was formed with life-off o f Ti/Au . A scanning electron microscopy (SEM) photograph of a finished device with overlapping gate is shown in Figure 5.2. Details o f the fabrication process are described in Appendix A. Figure 5.2: Top view o f a finished device showing the overlapping gate metals on the LTG-Alo.3 Gao.7 As passivation; the gate geometry is 1.2 pm foot-print with a 2 pm overlapping metal. 72 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. 5.3 Device Result and Analysis: 5.3.1 DC Characteristics Upon completion o f processing, devices were probed and characterized onwafer. DC measurement were done using an HP-4145B Parameter Analyzer. The gate-drain diode characteristics for both the LTG-Alo.3 Gao.7 As passivated FET and that o f the control sample is shown in Figure 5.3. As expected, the LTGAIo.3 Gao.7 As device has twice the breakdown voltage as compared to that of the control, with undoped Alo.3 Gao.7 As passivation. This reaffirmed that the LTGAlo.3 Gao.7 As passivation layer does indeed act as an effective charge absorber; and alleviated the peak gate electric field for the HFET structure. In addition, the reverse leakage current shown in Figure 5.3 is much lowered than that of LTG-GaAs passivation [6 ], this is attributed to the large band-gap o f the Aio.3 Gao.7 As spacer placed underneath the gate metal. The low reverse leakage current is desirable in power MESFET because it would led to an enhancement o f the power conversion efficiency in the device (i.e. high power-added-efficiency) . 73 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. s a a 0.5 o n BV - 20 V c v u u 3 u BV - 1 0 V LTG-Passivated -0.5 3 O C ontrol -25 -20 -15 -10 Gate V oltage [V] Figure 5.3: Gate-drain diode characterisitics of high-power LTG-AIo.3 Gao.7 As passivated GaAs HFET, the device gate foot-print is 1.2 pm, with 5 pm sourcedrain spacing. The control device had similar epistructure except that the LTGAlo.3 Gao.7 As is replaced with undoped Alo.3 Gao.7 As. Figure 5.4 displays a nominal current-voltage characteristics of the device. The maximum drain current at a gate forward bias of 0.5 V is about 480 mA/mm. The transconductance o f the device is about 140 mS/mm, which is about 40% higher than typical GaAs MESFET [8 ] (and also those presented in Chapter 4). The enhanced transconductance is due to the improved channel conductance associated with heterostructure. The improved device transconductance is sought after because it usually manifested in higher power gain for the device in power application , 74 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. 700 600 ~ 500 -I < £ 400 s g = 140 mS/mm V = - 0.5 V 300 200 100 Vd s (V) 1 ' Figure 5.4: Current-voltage characteristics o f a 1.2 pm gate-length LTGAlo.3 Gao.7 As passivated HFET. The device “on-state” breakdown voltage, defined as the drain breakdown voltage with the channel fully opened is ~10V. This high on-state breakdown voltage is attributed to the suppression of hole injection from the contacts through the use o f non-alloyed MOCVD regrown contacts. In order to verify this, we have also fabricated a device with normal alloyed contacts. The I-V characteristics is shown in Figure 5.5. The on-state breakdown voltage is clearly lowered while all other device figures-of-merit are similar to that o f the non-alloyed contacts device. 75 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. 0.1 4 5 0 °C ~>J ~ < 0.08 420 1u 0.06 U 1 No Annealing 0.04 2 ° 0.02 0 2 4 6 8 10 Drain Voltage (V) Figure 5.5: On-state breakdown voltage dependence on annealing temperatures of ohmic conctacts. 5.3.2 RF Characteristics Small signal measurements using an HP-851 OB automatic network analyzer were performed on the passivated device. A nominal frequency performance as a function o f gate bias, with a drain bias o f 5V, is shown in Figure 5.6. The unity current gain cut-off frequency (fj) of -7 GHz were obtained throughout the gate bias range. The unity power gain cut-off frequency (fmax) showed a stronger gate bias dependence, with fmax = 20 GHz at the gate bias o f -IV. These high frequency figures-of-merit indicated that the device should be able to perform as a microwave power amplifier. 76 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. 25 20 m ax 15 g 10 5 0 -4 2 3 -1 0 Gate Bias (V) Figure 5.6: Frequency performance as a function o f gate bias of an LTGAlo.3 Gao.7 As HFET with 1.2 pm gate foot-print (2 pm overlapping gate). 5.3.3 Microwave Power Performance The device characteristics discussed above showed promises for potential high power performance. On-wafer continuous-wave power measurements were performed at 4 GHz for a 400 pm wide device. Class-A biasing at a source-drain voltage o f 12V and half of the maximum drain current (Id = 50% Imax) was used for the measurement. The device delivered a maximum output power of 1.0 W/mm at 30% PAE (Power-Added-Efficiency) was achieved. The linear gain of the device is 11.5 dB. Figure 5.7 displays the output power and power added efficiency of the device at 4 GHz. 77 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. 30 50 1 :W /m m 4 0 3 0-j > ts 20 ^ 1 0 5 -5.0 -t0.0 . j— 5 .0 P, I n 10.0 [dBm ] ............ 15.0 o 20.0 Figure 5.7: Continous-wave power performance of a 1.2 pm gate length LTGAlo.3 Gao.7 As passivated HFET at 4 GHz. Upon timing the load for high PAE, a PAE o f 46% with an output power of 0.5 W/mm was achieved (Figure 5.8). Higher frequency measurement was also performed and is displayed in Figure 5.9. At 8 GHz, the device in Class-A bias (Vds=9 V and Vgs=-1.3V) delivered 825 mW/mm at 27% PAE, with a linear gain of 6.5dB. 78 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. 30 100 E ■o 80 4 GHz 2 5 > S3 2 0 ’S 1 5 20 1 0 0 5 0 1 5 1 0 25 2 0 P.in [dBm] Figure 5.8 : Performance characteristics o f an LTG-Alo.3 Gao.7 As passivated HFET was tuned for high power-added-efficiency (PAE) at 4 GHz. 30 50 P 25 s a T3 = 8 2 5 mW/miB 8 GHz 4 40 20 30 , > 15 P3 Gain ~ 6.5 dB L 20 10 £ 10 5 0 0 ; 10 15 0 20 P [dBm] Figure 5.9 : Power performance of an LTG-AlojGao 7 AS passivated HFET at GHz. 79 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. 8 5.4 S um m ary •' In this chapter, a high performance GaAs-based microwave power FET has been demonstrated. The device incorporated an LTG-Alo.3 Gao.7 As passivation layer in an HFET channel structure. The device characteristics and performance provided convincing testimony to the suitibility of the LTG-Alo.3 Gao.7 As passivation technology for GaAs-based power field effect transistor. A high-power FET fabrication process, which utilized non-alloyed selective regrown contacts by MOCVD and an overlapping gate structure, and is compatible with LTGAlo.3 Gao.7 As passivation have been developed. High performance devices utilizing this process have been realized and demonstrated. A maximum output power density of 1.0 W/mm was obtained with an LTG-Alo.3 Gao.7 As passivated HFET, and a high PAE of 46% was achieved when the device was tuned for high efficiency. These results are among the best reported values for GaAs-based FET . 80 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. 5.5 References :  F. W. Smith, C. L. Chen, L. J. Mahoney, M. J. Manfra, D. H. Temme, B. J. Clifton, and A. R. Calawa, “A 1.57 W/mm GaAs-based MISFET for highpower and microwave-switching applications,” 1991 IEEE MTT-S International Microwave Symposium Digest (91CH2870-4), Vol. 2, pp. 643646, 1991.  P. H. Ladbrooke, MMIC Design: GaAs FETs and HEMTs. Boston London: Artech House Inc., 1989.  Y. Aokie and Y. Hirano, High-power GaAs FETs. Boston London: Artech House Inc., 1993.  N. X. Nguyen, J. P. Ibbetson, J. C. Yen, M. H. Hashemi, and U. K. Mishra, “Encapsulated GaAs power MESFET.,” Proceedings. IEEE/Cornell Conference on Advanced Concepts in High Speed Semiconductor Devices and Circuits (Cat. No.93CH3235-9), pp. 539-47, 1993.  C.-L. Chen, L. J. Mahoney, M. J. Manfra, F. W. Smith, D. H. Temme, and A. R. Calawa, “High-breakdown-voltage MESFET with a low-temperaturegrown GaAs passivation layer and overlapping gate structure,” IEEE Electron Device Letters, Vol. 13, pp. 335-337, 1992. [6 ] L.-W. Yin, “GaAs Based Power Transistor Utilizing Low-Temperature GaAs Grown by MBE as the Surface Insulator,” : University of California. Santa Barbara, 1992.  H. Fukui, S. H. Wemple, J. C. Irvin, W. C. Nehaus, J. C. M. Hwang, H. M. Cox, W. O. Schlosser, and J. V. DiLorenzo, “Reliability o f power GaAs 81 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. field-effect transistors,” IEEE Transactions on Electron Devices, Vol. 29, pp. 395-401, 1982. [8 ] S. M. Sze, Physics o f Semiconductor Devices. New York: John Wiley & Sons Inc., 1981.  A. Higashisaka, Y. Takayama, and F. Hasegawa, “A high-power GaAs MESFET with an experimentally optimized pattern,” IEEE Transactions on Electron Devices, Vol. 27, pp. 1025-1029, 1980. Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. CHAPTER 6 Summary and Future Work Sum m ary: The principal objective o f the present research has been to investigate the feasibility and potentials o f the application o f low temperature grown materials in surface engineering of GaAs devices and materials, as well as to gain a physical understanding into the mechanism that surface passivation with LTG materials has provided in improving the gate-drain breakdown voltage and hence the power performance of passivated devices. From a technological standpoint, LTG materials passivation presents a new technology in the continual search for an effective electrical surface passivation for GaAs devices and materials. Although further progresses and investigations are needed before the growth o f LTG materials can become reliable and reproducible; the high controllability associated with MBE growth, promises LTG materials passivation to be a potentially more stable technology for devices. The existence of excess As, hence high deep acceptor and deep donor concentrations, in the LTG layers make the materials unique. Furthermore, the strong dependence o f these concentrations on synthesis process, such as growth and annealing temperatures, enabled the materials to be readily engineered for specific device applications. We have demonstrated the device application o f LTG-Alo.3 Gao.7 As passivation in GaAs FET to improve the breakdown voltage. A systematic study of 83 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. the effects o f growth and annealing temperatures o f the LTG-Alo.3 Gao.7 As passivation layer on the gate-drain breakdown voltage o f the FET have been performed. We have also performed preliminary investigation on the effects of LTGAlo.3 Gao.7 As processing parameters on MESFET low-frequency noise characteristics o f the passivated devices. Proper LTG-Alo.3 Gao.7 As passivation has been observed to dramatically lower the low-frequency noise o f the FET. Drawing from the present knowledge of the material properties of LTGGaAs, we have proposed a physical model that would explain the observed improvement in the breakdown voltage arose from devices passivated with LTG materials. The model o f compensated deep donors hypothesized that, with LTG materials passivation, the empty states of the compensated deep donors which enabled the LTG material passivation layer to act as an effective charge absorber and alleviate the peak electric field at the drain-edge of the gate metal in a FET structure. Two dimensional electrostatic simulation using this model of LTG materials clearly confirmed that the deep acceptors concentration (which is equivalent to the compensated deep donors concentration, when Nd » Na) dramatically effect the breakdown voltage of the device. We have developed a thermally stable device fabrication process that has enabled us to systematically study the effect of growth and annealing temperatures on the characteristics o f LTG-Alo.3 Gao.7 As devices. The effect o f annealing of LTG materials is equivalently to the changing of defect concentrations in the LTG layer; 84 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. and this was experimentally demonstrated to have a clear impact on the breakdown voltages and other device characteristics. Device with record breakdown voltage of -40 V and maximum drain current o f 420 mA/mm has been demonstrated as convincing testimony to the potential o f the LTG material passivation technology. These results are substantially higher than those obtained with the current technology in the industry for high breakdown, namely gate recess etching [ 1 , 2 ]. High performance GaAs-based power FET, which incorporated LTGAlo.3 Gao.7 As passivation have also been demonstrated with record performance of 1 .0 W/mm at 30% Power-Added-Efficiency(PAE), and 0.5 W/mm at 46% PAE (at 4 GHz). This experimental result provided clear proof of the applicability o f the LTG-Alo.3 Gao.7 As passivation technology for microwave power devices. However, there are still other issues that needed consideration and investigation before the LTG materials passivation technology could be truly termed low cost and be implemented in existing fabrication process of GaAs power FET. Suggestions for Future Work As the device results in Chapter 4 have clearly demonstrated, the exact growth temperature of the LTG materials has critical impacts on the device characteristics, a difference in growth temperatures of ~25',C resulted in drastically difference device characteristics. However, this has been a fundamental in LTG materials research: a lack of a good method to precisely measure growth temperature 85 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. near 200°C. Recent developments in MBE technology have shown that the solution for more accurate low temperature measurements is possible in the immediate. Implementation o f such technology is a must for LTG materials growth, and it should lead to more reproducible LTG materials and device characteristics. The stability and reliability o f LTG passivated devices also needs more investigation. In particular, thermal stability of the LTG materials requires systematic study and characterization. These studies should be the final tests o f the suitability o f LTG materials passivation in GaAs power FET. In addition, implementation o f LTG materials passivation to other surface sensitive FET structures, such as low In composition ( <20% ) GaAs Pseudomorphic High Electron Mobility Transistor (PHEMT), would lead to improved power performance at high frequency with low cost, the combination that has been the much sought after by the emerging wireless communications industry. A high-power PHEMT structure, with large barrier (Alo.4 3 Gao.5 7 As) and high current capability (larger AEc and tellurium doping) have recently been demonstrated . Application of the LTG-Alo.3 Gao.7 As passivation technology to this device structure would lead to potentially high performance microwave power devices. 86 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission. References :  T. Furutsuka, T. Tsuji, and F. Hasegawa, “Improvement of the drain breakdown voltage o f GaAs power MESFETs by a simple recess structure,” IEEE Transactions on Electron Devices, Vol. 25, pp. 563-567, 1978.  T. Furutsuka, A. Higashisaka, Y. Aono, Y. Takayama, and F. Hasegawa, “GaAs power MESFETs with a graded recess structure,” Electronics Letters, Vol. 15, pp. 417-418, 1979.  N. X. Nguyen, W.-N. Jiang, K. A. Baumann, and U. K. Mishra, “Highbreakdown AlGaAs/InGaAs/GaAs PHEMT with tellurium doping.,” Electronics Letters, Vol. 31, pp. 586-568, 1995. 87 Reproduced with permission of the copyright owner. Further reproduction prohibited without permission.